Spreadsheet: 75051d1275573783-conditional-equations-example-9
Sheet: Raw_Material_Pigment_Listing

Legend: Blue is for discontinued pigments,orange is for experimental pigments and yellow is just to aid readability. H is for HIDM, F for FCM, E for polyethylene, V for EVA, S for polystyrene, M for EMA, and A for additives.
Intermediate Code | Product Code | Description | Color Index | Pigment Loading | Processing Equipment | Lot Number/ Location | Heat Stability (deg C) | Light Fastness | Compliance | Shade | Maximum Loading | Others
B500105 | B500105 | 50 MI LLDPE | NA | 1 | RESIN
B500118 | B500118 | FDA HDPE 8 MI | NA | 100^% | RESIN
B500124 | B500124 | EVA | NA | 1 | RESIN
B500128 | B500128 | GP LDPE | NA | 1 | RESIN
[NAME] | [NAME] | 10 MI LDPE | NA | 1 | RESIN
[NAME] | [NAME] | FDA EMA (G)  (6MI 21% MA) | NA | 1 | [NAME]
B500192 | B500192 | 20 MI RESIN | NA | 1 | RESIN
B500195 | B500195 | [NAME] | NA | 1 | RESIN
B500201 | B500201 | 2 MI LLDPE | NA | 1 | RESIN
B500313 | B500313 | PP (G), GEN.PURPOSE, 10-16 MFR | NA | 1 | RESIN
B500321 | B500321 | HUNTSMAN 13M11A COPP (G) | NA | 1 | RESIN
B500401 | B500401 | Nova 5511 HIPS (G)  (Old 5500) | NA | 1 | RESIN
B500408 | B500408 | MIPS, 12-20 MFR | NA | 1 | RESIN
2RM RESIN | B500XXX | HDPE BF RESIN | NA | 1 | RESIN
100FE05 | B601100 | TiO2 2073 (chloride) | PW6 | 0.05 | FCM |  | 1000 | High | FDA, [NAME] | Yellow | 75% | Use for colormatching regular colors. Do not use for: Extrusion Coating, Outdoor application (>1.5 Years), Fibers,
100FE20 | B601100 | TiO2 2073 (chloride) |  | 0.2 | FCM
100HE01 | B601100 | TiO2 2073 (chloride) |  | 0.01 | HIDM | 10/30/08
100HE05 | B601100 | TiO2 2073 (chloride) |  | 0.05 | HIDM | 10/30/08 / A1
100HE50 | B601100 | TiO2 2073 (chloride) |  | 0.5 | HIDM | A2
100HE70 | B601100 | TiO2 2073 (chloride) |  | 0.7 | HIDM
100HM05 | B601100 | TiO2 2073 (chloride) |  | 0.05 | HIDM | A1
100HS05 | B601100 | TiO2 2073 (chloride) |  | 0.05 | HIDM
N/A | B601101 | Titanox 1000 (Anatase TiO2) | PW6 | N/A | N/A |  | 1000 | Medium | FDA, [NAME] | Yellow | 50% | DO NOT USE THIS TiO2. For indoor application only.
N/A | D-B601102 | D-Lithopone (BaSO4/ZnS) | NA | N/A | N/A |  | 300 | Medium | [NAME] | Dirty Yellow | 40% | **DONOT USE**.White extender.
N/A | D-B601104 | [NAME] ([NAME]) | NA | N/A | N/A |  | 260 | Poor | Non-FDA, [NAME] | Off-white | 30-40% | **DONOT USE** White Extender
N/A | B601105 | Zoco 100 Zinc Oxide | NA | N/A | N/A |  | 260 | Poor | non-FDA, [NAME] | off-white | 30-40% | **DONOT USE**.White extender.
106FE05 | B601106 | Dupont R-960 TiO2 | PW6 | 0.05 | FCM | A2 | 800 | High | FDA | Blue | 70% | Use for outdoor application only, where life expectancy of part is greater than 3 years. 12% weaker than TiO2 2073 and 8% weaker than white 2220.
106HE05 | B601106 | Dupont R-960 TiO2 |  | 0.05 | HIDM
106HE50 | B601106 | Dupont R-960 TiO2 |  | 0.5 | HIDM | A2
106HM50 | B601106 | Dupont R-960 TiO2 |  | 0.5 | HIDM | A3
N/A | B601107 | Zoco 104 Zinc Oxide | NA | N/A | N/A |  | 260 | Poor | Non-FDA, [NAME] | Off-white | 30-40% | **DONOT USE**.White extender.
N/A | B601108 | [NAME] 2400 TiO2 | PW6 | N/A | N/A |  | 1000 | High | FDA, [NAME] | Blue | 75% | DISCONTINUED - USE DUPONT R104 - Use for extrsuion coating and fiber application. This TiO2 has better dispersion and rheological characteristics than the B601100
109HE05 | B601109 | [NAME] 2220 TiO2 | PW6 | 0.05 | HIDM |  | 1000 | High | FDA, [NAME] | Blue | 70% | Use for semi-wheaterable applications, where outdoor exposure is between 1 and 3 years.
109FE05 | B601109 | [NAME] 2220 TiO2 |  | 0.05 | FCM | A3
N/A | [NAME] | [NAME] | PW6 | N/A | N/A |  | 1000 | High | FDA, [NAME] | Blue | 70% | DO NOT USE THIS PIGMENT UNLESS SPECIFIED. Use B601106
N/A | B601111 | [NAME] | PW6 | N/A | N/A |  | 1000 | High | FDA, [NAME] | Blue | 70% | Only use this pigment when the B601113 is not readily available
N/A | B601112 | RCL 4 TiO2 | PW6 | N/A | N/A |  | 600 | Medium | FDA, [NAME] | Blue | 70% | Only use this pigment when the B601113 is not readily available
113HE05 | B601113 | Dupont R-104 TiO2 | PW6 | 0.05 | HIDM | A3 | 600 | High | FDA | Bluer than 2073 | 85% | Use this TiO2 for extrusion Coating Application - Use instead of [NAME] 2400 B601108 -. Extremelly good dispersion characteristics.
113HE70 | B601113 | Dupont R-104 TiO2 |  | 0.7 | HIDM | A4
N/A | D-B601115 | D-Anatase G/P 1014 TiO2 | PW6 | N/A | N/A |  | 1000 | High | FDA, [NAME] | Blue | 50% | Use for Utility colors where pricing is an issue. Do not use for outdoor application
N/A | D-B601116 | D-TiO2 GP | PW6 | N/A | N/A |  | 600 | High | FDA | Same as 2073 | 70 | Use only for General Purpose or Utility Applicatios. Dispersion quality of this pigment is questionable. Use only when specified in LRN
N/A | D-B601118 | D-UV Titan P160 UF TiO2 | PW6 | N/A | N/A |  | 260 | Excellent | Non-FDA, [NAME] | Blue | 30-40% | This is a Ultra Fine (UF) TiO2. Use as an UV absorber for agricultural or green house film applicatio. Do not use for colour mathing
N/A | B601120 | TR-28 TiO2 | PW6 | N/A | N/A |  | 600 | High | FDA | Blue | 70% | Do not use unless specified to do so.
N/A | B601121 | APG TiO2 | PW6 | N/A | N/A |  | 800 | Medium | FDA | Blue | 70% | Eastman Kodak anataseTiO2. Do not use unless advised to do so.
124HE05 | D-B601124 | D-Titan 10/R03 [NAME] | PW6 | 0.05 | HIDM |  | 280 | High | FDA | Yellow | 50-70 | Primary TiO2 for low cost application. Keep the temperature in mind. DONOT use for critical application(such as extrusion coating ect...)
124HE50 | D-B601124 | D-Titan 10/R03 [NAME] |  | 0.5 | HIDM | A4
134HE25 | B601134 | Iriodin 163 Shimmer Pearl | NA | 0.25 | HIDM | A5 | 500 | High | FDA | Yellow | 20% | Particle size 20-180 microns
N/A | B601136 | Iriodin 120 [NAME] | NA | N/A | N/A |  | 500 | High | FDA | Yellow | 20% | **DONOT USE**
N/A | D-B601137 | D-Iriodin 119 Polar White | NA | N/A | N/A |  | 500 | High | FDA | Yellow | 20% | *Use B601147 instead*  Particle size 5-25 microns
138HE20 | D-B601138 | D-Iriodin 153 Flash Pearl | NA | 0.2 | HIDM | A5 | 500 | High | FDA | Yellow | 20% | *DISCONTINUED DO NOT USE* USE B601153 INSTEAD
N/A | B601139 | Iriodin 123 Bright Luster | NA | N/A | N/A |  | 500 | High | FDA | Yellow | 20 | *Use B601147 instead * Particle size 5-25 microns
N/A | D-B601140 | D-Iriodin 110 Fine Satin | NA | N/A | N/A |  | 500 | High | FDA | Yellow | 20 | *DISCONTINUED DO NOT USE* USE B601155 INSTEAD
N/A | B601141 | Flonac MF 11 | NA | N/A | N/A |  | 500 | High | FDA | Yellow | 20 | *Use B601147 instead*  Particle size 5-25 microns
N/A | D-B601142 | D-Preblend [NAME] | NA | N/A | N/A |  | 500 | High | FDA | Yellow | 60 | **DONOT USE**This is the compacted version of the B601141 and B601139. It contains 80& mica, A/0 and [NAME].
N/A | B601146 | Iriodin 109 Glacier White | NA | N/A | N/A |  | 500 | High | FDA | Yellow | 30% | *Use B601147 instead* Particle size 5-60 microns
147HE25 | [NAME] | 280-1103 Sunmica 41127 TCM WH | N/A | 0.25 | HIDM | A6 | 500 | high | FDA, [NAME] | Yellow | 30 | *Use as your primary mica*
147HE10 | [NAME] | 280-1103 Sunmica 41127 TCM WH |  | 0.1 | HIDM
147HE01 | [NAME] | 280-1103 Sunmica 41127 TCM WH |  | 0.01 | HIDM
147HS20 | [NAME] | 280-1103 Sunmica 41127 TCM WH |  | 0.2 | HIDM | A5
147HV25 | [NAME] | 280-1103 Sunmica 41127 TCM WH |  | 0.25 | HIDM | A6
148HE20 | D-B601148 | D-Iriodin 119 WM8 | N/A | 0.2 | HIDM | A6 | 300 | High | FDA, [NAME] | YELLOW | 50 | *DISCONTINUED DO NOT USE* USE B601156 INSTEAD
153HE25 | [NAME] | [NAME] | N/A | 0.25 | HIDM |  | 600 | High | FDA | Yellow | 0.25
153HE10 | [NAME] | [NAME] |  | 0.1
153HE01 | [NAME] | [NAME] |  | 0.01
154HE25 | B601154 | [NAME] | N/A | 0.25 | HIDM |  | 600 | High | FDA | Yellow | 0.25
154HE10 | B601154 | [NAME] |  | 0.1
154HE01 | B601154 | [NAME] |  | 0.01
155HE25 | B601155 | [NAME] TZ1006A | N/A | 0.25 | HIDM |  | 600 | High | FDA | Yellow | 0.25
155HE10 | B601155 | [NAME] TZ1006A |  | 0.1
155HE01 | B601155 | [NAME] TZ1006A |  | 0.01
 | B601156 | TAIZHU  MICA TND1222 | NA |  | HIDM |  | 300 | HIGH | FDA | YELLOW | 50 | THIS IS A FREE FLOW MICA ALREADY ENCAPSULATED IN PE. THIS SHOULD BE USED WHEN NEEDING MATERIAL AT GREATER THAN 25% POWDER MICA
N/A | D-B601200 | D-V-9415 Yellow | PY53 | N/A | N/A |  | 1000 | High | Non FDA, [NAME] | Green | 30-35% | **DONOT USE UNLESS SPECIFIED** Same color as B601231 Yellow 195.
N/A | D-B601201 | D-Cadmium Yellow P-11101 | 77205 | N/A | N/A |  | 300 | high | Heavy Metal based | red | as needed | *DONOT USE*
N/A | D-B601202 | D-'C71-5171 D&C Yellow#10 | 47005:1 | N/A | N/A |  | 260 | low | FDA, [NAME] | Mid green-red | 7-10% | *CUSTOMER SPECIFIED PIGMENT* Donot use unless specified
203FE01 | B601203 | PV Fast Yellow HR 02 | PY 83 | 0.01 | FCM | 10/2/06 / A8 | 200 | low | NON FDA,Diarylide, [NAME] | red | 8 - 10 | Same color as B601259 Yellow 275-0570.  Donot use for outdoor application
203FE07 | B601203 | PV Fast Yellow HR 02 |  | 0.07 | FCM/Prod. Made | CNDA501790/0110
203FE10 | B601203 | PV Fast Yellow HR 02 |  | 0.1 | FCM | DEBF139839 / A8
203HE01 | B601203 | PV Fast Yellow HR 02 |  | 0.01 | HIDM
203HE07 | B601203 | PV Fast Yellow HR 02 |  | 0.07 | HIDM | CNDA501790/0110
203HE10 | B601203 | PV Fast Yellow HR 02 |  | 0.1 | HIDM | A8
204FE01 | D-B601204 | D-Graphtol Yellow GR | PY 13 | 0.01 | FCM | 10/2/06 | 200 | low | NON FDA,Diarylide, [NAME] | Mid  green-red | 8 - 10 | *DISCONTINUED DO NOT USE* USED B602217 INSTEAD
204FE10 | D-B601204 | D-Graphtol Yellow GR |  | 0.1 | FCM | DEBF001906 / A9
204HE01 | D-B601204 | D-Graphtol Yellow GR |  | 0.01 | HIDM | A9
204HE10 | D-B601204 | D-Graphtol Yellow GR |  | 0.1 | HIDM | A9
205FE05 | B601205 | [NAME] TiO2 | NA | 0.05 | FCM | 10/2/06 / A10 | 600 | High | FDA, [NAME] | Yellow Shade TiO2 | As required | Use as much as possible to reduce cost in formulas by replacing white, yellow or green pigments. 20% less opacity than regular TiO2.
205FE10 | B601205 | [NAME] TiO2 |  | 0.1 | FCM
205HE50 | B601205 | [NAME] TiO2 |  | 0.5 | HIDM | A10
206HE01 | D-B601206 | D-Yellow Iron Oxide 2087 | Y42 | 0.01 | HIDM | A10 | 225 | High | FDA, [NAME] | Green | 40-45% | Do not use for injection molding. Similar color to B601213. PIGMENT TURNS RED  WHEN IT DEGRADES *USE B601294 INSTEAD*
206HE10 | D-B601206 | D-Yellow Iron Oxide 2087 |  | 0.1 | HIDM | A10
N/A | D-B601207 | D-Cromophtal Yellow GT-AD | PY 199 | N/A | N/A |  | 300 | High | FDA, [NAME] | red | 10 - 12 | *DONOT USE*
208HE01 | D-B601208 | D-388X W/S Yellow Iron Oxide |  | 0.01 | HIDM | A11
208HE10 | D-B601208 | D-388X W/S Yellow Iron Oxide |  | 0.1 | HIDM | A11
209HV10 | D-B601209 | D-ZQ-17 Saturn Yellow | N/A | 0.1 | HIDM | A11 | 300 | low | Non FDA, [NAME] | green | 50 | **DISCONTINUED DO NOT USE**  USE B602214                                                    Do not use Zn-St or [NAME] in combination with this pigment. Melting point of polyamide carrier resin is 175C. Need to run 175C or higher for develop color.
209HV25 | D-B601209 | D-ZQ-17 Saturn Yellow |  | 0.25 | HIDM | A11
N/A | D-B601212 | D-Colortherm 20 Yellow I.O. | Y42 | N/A | N/A |  | 260 | High | Non-FDA, [NAME] | Green | 40-45% | *DISCONTINUED. DONOT USE* Use B601214 instead
213FE01 | D-B601213 | D-Bayferrox 3420 Yellow Iron oxide | Y42 | 0.01 | FCM | Jan./06 / A11 | 220 | High | FDA, [NAME] | Green | 40-45% | Do not use for Injection molding; [NAME] in to yellow 2087. PIGMENT TURNS RED WHEN IT DEGRADES *USE B601294 INSTEAD*
213HE01 | D-B601213 | D-Bayferrox 3420 Yellow Iron oxide |  | 0.01 | HIDM
213HE10 | D-B601213 | D-Bayferrox 3420 Yellow Iron oxide |  | 0.1 | HIDM | A12
214FE01 | D-B601214 | D-Colortherm 10 Yellow Iron Oxide | Y42 | 0.01 | FCM | Jan./06 / A12 | 260 | High | FDA, [NAME] | Green | 35-45% | Heat stable version of [NAME], and FDA version of B601212. PIGMENT TURNS RED  WHEN IT DEGRADES  *USE B601296 INSTEAD*
214HE01 | D-B601214 | D-Colortherm 10 Yellow Iron Oxide |  | 0.01 | HIDM
214HE10 | D-B601214 | D-Colortherm 10 Yellow Iron Oxide |  | 0.1 | HIDM | A12
214HE50 | D-B601214 | D-Colortherm 10 Yellow Iron Oxide |  | 0.5 | HIDM | A12
214HS20 | D-B601214 | D-Colortherm 10 Yellow Iron Oxide |  | 0.2 | HIDM | A13
12902C18 | 12902C18 | YELLOW 10 DRY BLEND |  | 0.05 | Powder Intermediate
218HV10 | D-B601218 | D-ZQ-16 Arc Yellow | NA | 0.1 | HIDM | A13 | 300 | Poor | Non-FDA, [NAME] | Red [NAME] | 30-40% | **DO NOT USE - DISCONTINUED**  USE B602215                                                 Do not use [NAME] or CaSt in combination with this pigment. Melting point of the polyamide carrier resin is 175C, We must meet Melting point in order to develop the color.
218HV25 | D-B601218 | D-ZQ-16 Arc Yellow |  | 0.25 | HIDM | A13
219HE25 | B601219 | Microlen [NAME] (Flush) | 168 | 0.25 | HIDM | A13 | 240 | Low-Medium | Non-FDA, [NAME] | Green | 25% | Predispersed product with a 50% pigment loading. Use only when excellent dispersion is required
221FE01 | D-B601221 | D-PVFY HGR Yellow | 191 | 0.01 | FCM | DEBF022610, [NAME]  / A14 | 300 | Good-High | FDA | Red | 8 -12% | *Use B601268 instead*  FDA compliant to maximum of 1% pigment in final product.
221FE10 | D-B601221 | D-PVFY HGR Yellow |  | 0.1 | FCM | A14
221HE01 | D-B601221 | D-PVFY HGR Yellow |  | 0.01 | HIDM
221HE10 | D-B601221 | D-PVFY HGR Yellow |  | 0.1 | HIDM | A15
221HS01 | D-B601221 | D-PVFY HGR Yellow |  | 0.01 | HIDM | A14
221HS10 | D-B601221 | D-PVFY HGR Yellow |  | 0.1 | HIDM | A14
12904C18 | D-12904C18 | D-YELLOW HGR DRY BLEND | 191 | 0.05 | Powder Intermediate |  | 300 | Good-High | FDA | Red | 8-12% | *Use B601268 instead*  FDA compliant to maximum of 1% pigment in final product.
225FE01 | D-B601225 | D-PVFY HG Diazo Yellow | 180 | 0.01 | FCM | DALA015053 / A15 | 290 | Good | FDA | Green | 8-12% | *DISCONTINUED DO NOT USE* USE B602211 INSTEAD
225FE10 | D-B601225 | D-PVFY HG Diazo Yellow |  | 0.1 | FCM | A16
225HE01 | D-B601225 | D-PVFY HG Diazo Yellow |  | 0.01 | HIDM | A16
225HE10 | D-B601225 | D-PVFY HG Diazo Yellow |  | 0.1 | HIDM | A16
120LC002 | D-120LC002 | D-PVFY HG Diazo Yellow Dryblend Intermediate |  | 0.05 | Powder Intermediate
228HE01 | B601228 | 5GNO1 Bayplast Yellow | 150 | 0.01 | HIDM | A17 | 300 | High | Non-FDA, [NAME] | Green, Dirty | 10-15% | Very strong, high heat stability and lightfastness.
228FE01 | B601228 | 5GNO1 Bayplast Yellow |  | 0.01 | FCM | E19001/1, 10/2/06  / A16
228FE10 | B601228 | 5GNO1 Bayplast Yellow |  | 0.1 | FCM | E19001/1 / A17
230FE01 | B601230 | [NAME] Paliotol Yellow | 138 | 0.01 | FCM | 690158, 10/2/06 / A17 | 260 | high | FDA, [NAME] | Green | 10-12% | FDA compliant pigment, with an FDA limitation of 1% pigment in the final part. Not as strong as yellow HG
230FE10 | B601230 | [NAME] Paliotol Yellow |  | 0.1 | FCM | 080019P050 / A18
230HE01 | B601230 | [NAME] Paliotol Yellow |  | 0.01 | HIDM | A18
230HE10 | B601230 | [NAME] Paliotol Yellow |  | 0.1 | HIDM | A18
230FS05 | B601230 | [NAME] Paliotol Yellow |  | 0.05 | FCM | 080019P050 / A18
120LC029 | 120LC029 | YELLOW K0961D DRY BLEND |  | 0.05 | Powder Intermediate
231HE10 | D-B601231 | Yellow 195 Nickel Titanate | 53 | 0.1 | HIDM | A19 | 300 | High | Non-FDA, [NAME] | Green | 30-35% | Very weak pigment, washout green shade
N/A | D-B601232 | GR Chromophtal Yellow | 95 | N/A | N/A |  | 260 | Good-High | FDA | Green | 10-15% | *DONOT USE*
233FE10 | D-B601233 | D-3GP Graphtol  Fast Yellow | 155 | 0.1 | FCM | A19 | 220 | Moderate-Good | Non-FDA, [NAME] | Green | 8-12% | *DISCONTINUED DO NOT USE* USE B602212 INSTEAD
233HE10 | D-B601233 | D-3GP Graphtol  Fast Yellow |  | 0.1 | HIDM | A19
12903C18 | [NAME] | D-YELLOW 3GP DRY BLEND |  | 0.05 | Powder Intermediate
N/A | D-B601234 | D-Cromophtal Yellow HRP | 191:1 | N/A | N/A |  | 300 | High | Non-FDA, [NAME] | Red | 8-10% | *DO NOT USE*
235FE10 | D-B601235 | D-1364 [NAME] yellow | 62 | 0.1 | FCM | A20 | 250 | Moderate-Good | Non-FDA, [NAME] | Red | 12-16% | Very similar to Yellow WSR but stronger. Dispersion is a concern
235HE10 | D-B601235 | D-1364 [NAME] yellow |  | 0.1 | HIDM | A20
236FE01 | B601236 | 279-5700 Fanchon  Yellow | 139 | 0.01 | FCM | A20 | 280 | High | Non-FDA, [NAME] | Red | 8-12% | Strong red shade pigment, high light fastness
236FE10 | B601236 | 279-5700 Fanchon  Yellow |  | 0.1 | FCM | A21
236HE01 | B601236 | 279-5700 Fanchon  Yellow |  | 0.01 | HIDM | A21
236HE10 | B601236 | 279-5700 Fanchon  Yellow |  | 0.1 | HIDM | A21
237FE01 | B601237 | [NAME] | 168 | 0.01 | FCM | A22 | 240 | Low-Medium | Non-FDA, [NAME] | Green | 12-16% | ** USE B602213 DCC YELLOW 1368 IF WGP IS UNAVAILABLE**
237FE10 | B601237 | [NAME] |  | 0.1 | FCM | 90147FW8 / A22
237HE01 | B601237 | [NAME] |  | 0.01 | HIDM | A21
237HE10 | B601237 | [NAME] |  | 0.1 | HIDM | A23
120LC060 | 120LC060 | [NAME]  Intermedaite |  | 0.05 | Powder Intermediate
238HE10 | D-B601238 | D-K1841 Paliotol Yellow | 139 | 0.1 | HIDM | 070066P040 / A23 | 240 | High | Non-FDA, [NAME] | Red | 8-12% | Similar to Y5700 yellow, but weaker. High lightfastness
239FE01 | D-B601239 | D-WSR [NAME] | 62 | 0.01 | FCM | Jan./06 / A23 | 250 | Low-Medium | Non-FDA, [NAME] | Red | 12-16% | *DISCONTINUED DO NOT USE* USE B602216 INSTEAD
239FE10 | D-B601239 | D-WSR [NAME] |  | 0.1 | FCM | A24
239HE01 | D-B601239 | D-WSR [NAME] |  | 0.01 | HIDM | A24
239HE10 | D-B601239 | D-WSR [NAME] |  | 0.1 | HIDM | A24
120LC030 | D-120LC030 | D-YELLOW WSR DRY BLEND |  | 0.05 | Powder Intermediate
240HE05 | D-B601240 | D-1003 [NAME] (PbCr) | 34 | 0.05 | HIDM | B1 | 230 | Good ([NAME] 1 year) | Heavy Metal Based (Lead) | Red | 80 | DO NOT USE for IM or High Heat Application                        *DISCONTINUED DO NOT USE* USE B602219 INSTEAD
240HE50 | D-B601240 | D-1003 [NAME] (PbCr) |  | 0.5 | HIDM | B1
241HE05 | D-B601241 | D-1032 Lemon [NAME] (PbCr) | 34 | 0.05 | HIDM | B1 | 230 | Good ([NAME] 1 year) | Heavy Metal Based (Lead) | Clean Green | 80 | DO NOT USE for IM or High Heat Application                *DISCONTINUED DO NOT USE* USE B602220 INSTEAD
241HE50 | D-B601241 | D-1032 Lemon [NAME] (PbCr) |  | 0.5 | HIDM | B1
242FE05 | B601242 | 1080 Primrose [NAME] (PbCr) | 34 | 0.05 | FCM |  | 230 | Good(max 1 year) | Heavy Metal Based (Lead) | Green | 80 | *DONOT USE FOR IM* Greenest Shade. Always use [NAME] and B900 in formula
242HE05 | B601242 | 1080 Primrose [NAME] (PbCr) |  | 0.05 | HIDM
242HE50 | B601242 | 1080 Primrose [NAME] (PbCr) |  | 0.5 | HIDM | B1
243HE50 | D-B601243 | [NAME] [NAME] (PbCr) | 34 | 0.5 | HIDM | 06/24/09 - B1 | 230 | Good | Heavy Metal Based (Lead) | Red | 80% | *DONOT USE FOR IM*  Not heat stable [NAME] and B900 in formula *USE B602219 INSTEAD*
243HE05 | D-B601243 | [NAME] (PbCr) | 34 | 0.05 | HIDM | 06/24/09 - B1
N/A | B601244 | 1019 Yellow (PbCr) | Y34 | N/A | N/A |  | 260C | High | Heavy Metal - Lead Cromate | Red | 80 | DO NOT USE THIS PIGMENT.  USE THE B601240 1003 Yellow.
245HE50 | D-B601245 | D-1034 [NAME] (PbCr) | 34 | 0.5 | HIDM | 21025/060g | 260 | medium | Hemay Metal, Lead Chromate | Green | 60% | **DISCONTINUED - DO NOT USE'*  USE B602221  (THIS YELLOW 1034 IS CUSTOMER SPECIFIED PIGMENT -  DO NOT USE)
245HE05 | D-B601245 | D-1034 [NAME] (PbCr) | 34 | 0.05 | HIDM | 21025/060g
N/A | D-B601246 | D-KY907 Medium Crome Yellow | Y34 | N/A | N/A |  | 300 | High | Heavy Metal, Lead Chromate | Red | 50% | Heat stable pigment, similar in shade as the 1003  but 30% weaker due to the silica coating on the KY907 pigment. PROBLEMS WITH MOISTURE - USE WITH CARE
N/A | D-B601247 | D-KY908 Lemon Yellow | Y34 | N/A | N/A |  | 300 | High | Heavy Metal, Lead Chromate | Green | 50% | Heat stable pigment, similar in shade as the 1032 but 30% weaker due to the silica coating on the KY908 pigment. PROBLEMS WITH MOISTURE. USE WITH CARE
N/A | D-B601248 | D-1077 Primrose | Y34 | N/A | N/A |  | 220 | High | Heavy Metal, Lead Chromate | Green | 50% | DO NOT USE THIS PIGMENT - USE B601242 1080 YELLOW
N/A | D-B601249 | D-[NAME] | Y34 | N/A | N/A |  | 300 | High | Heavy Metal, Lead Chromate | Green | 50% | Heat stable pigment, similar in shade as the 1032 but 30% weaker due to the silica coating on the [NAME] pigment. PROBLEMS WITH MOISTURE. USE WITH CARE
250HE01 | D-B601250 | D-9609/C69-4537 FD&C Yellow #5 | FDC Yellow 5 | 0.01 | HIDM | B2 | 240 | Poor | FDA | Red | 8 - 12% | *DISCONTINUED DO NOT USE* USE B602218 instead. Low Bulk Density. For direct/inderect food contact application
N/A | D-B601251 | D-C70-5270 FD&C Yellow #6 | [NAME] | N/A | N/A |  | 260 | Poor | FDA | Red | 12-16 | *DONOT USE UNLESS SPECIFIED* Low Bulk Density. For direct/indirect food contact application
N/A | B601252 | 2GLTE Irgazin Yellow | 109 | N/A | N/A |  | 270 | High | Non-FDA, [NAME] | Green | 8 - 12% | Expensive Yellow. High Ligthfastness. Tends to Warp
253FE01 | D-B601253 | D-Cromophtal Yellow HRPA | PY 191:1 | 0.01 | FCM | Jan./06 / B2 | 300 | Good-High | FDA, [NAME] | red | 12 | Color same as B601221 yellow HGR but cost less. FDA compliant to maximum of 0.5% in final product.
254HE01 | B601254 | Light Fast yellow 6R | PBr 24 | 0.01 | HIDM | B2 | 1000 | High | FDA, [NAME] | Red | 40-45% | '*FDA Compliant to maximum of 2% pigment in final product.** Weak, inorganic FDA yellow. Use only when Colortherm 10 or 3950 can not be used due to tempertaure limitations.
254HE10 | B601254 | Light Fast yellow 6R |  | 0.1 | HIDM | B2
254HE50 | B601254 | Light Fast yellow 6R |  | 0.5 | HIDM | B2
255HE01 | D-B601255 | D-Bayferrox 415 Yellow Iron Oxide | Y42 | 0.01 | HIDM | B2 | 220 | Good | Non-FDA, [NAME] | Dirty Green | 40 - 42% | *USE B601276 YELLOW 3020 INSTEAD* Utility Iron Oxide Yellow. Weaker than 3420 and dirtier. PIGMENT TURNS RED  WHEN IT DEGRADES
N/A | D-B601256 | D-YL-3100 / YO-3100 / YB-2087 Yellow | Y42 | N/A | N/A |  | 200 | High | Non-FDA, [NAME] | Green | 40% | *DONOT USE* Utility Iron Oxide Yellow. Weaker than 3420 and dirtier. PIGMENT TURNS RED  WHEN IT DEGRADES. Use only for cheap film application
258HE10 | B601258 | L75-2377 Yellow Diarylide | 83 | 0.1 | HIDM | B3 | 200 | Low | Non-FDA, [NAME] | Red | 20 - 30 % | Flush version of 275-0570 contains 50% pigment. Limited Heat Stability. Donot use for outdoor application.
259HE10 | D-B601259 | D-275-0570 YELLOW DIARYLIDE | 83 | 0.1 | HIDM | B3 | 200 | low | Non-FDA, [NAME] | Red | 8 - 10% | Strong pigment, difficult to disperse. Limited heat stability. Donot use for outdoor application. Use B601203 for lower cost.
259FE10 | D-B601259 | 275-0570 Yellow Diarylide |  | 0.1 | FCM | 10/30/07 / B3
260HE10 | D-B601260 | D-275-0049 YELLOW DIARYLIDE | 13 | 0.1 | HIDM | B3 | 200 | low | Non-FDA, [NAME] | Mid Green-Red | 8 - 10% | Strong pigment, difficult to disperse. Limited heat stability. Donot use for outdoor application. Use B601204 for lower cost.
260FE01 | D-B601260 | D-275-0049 Yellow Diarylide |  | 0.01 | FCM | STD / B3
260FE10 | D-B601260 | D-275-0049 Yellow Diarylide |  | 0.1 | FCM | STD, 10/30/07 / B3
N/A | D-B601261 | D-313 Yellow Iron Oxide | 42 | N/A | N/A |  | 200 | Good | Non-FDA, [NAME] | Dirty Green | 40 - 45% | *DO NOT USE* EXTREMELLY POOR DISPERSION
262FE01 | D-B601262 | D-274-3954 Yellow Diarylide | 14 | 0.01 | FCM | Jan./06 / B4 | 210 | Low | Non-FDA, [NAME] | Green | 8 - 12% | *DISCONTINUED;  DO NOT USE* USE B602225 INSTEAD. Strong pigment, difficult to disperse. Limited heat stability. Donot use for outdoor application.
262FE10 | D-B601262 | D-274-3954 Yellow Diarylide |  | 0.1 | FCM | B4
262HE10 | D-B601262 | D-274-3954 Yellow Diarylide |  | 0.1 | HIDM
N/A | B601263 | L74-1357 Yellow Diarylide | 14 | N/A | N/A |  | 200 | Low | Non FDA, [NAME] | Green | 30-40% | This is the flush version of the 274-3954 green shade pigment. Pigment loading of this flush product is 50%. Use only when the maximum loading of the B601262 is reached.Donot use for outdoor application.
N/A | D-B601264 | [NAME] | 83 | N/A | N/A |  | 200 | Low | Non-FDA, [NAME] | Red | 6-8% | *DONOT USE* This is the color equivalent ot the B601259 275-070. The 1245 is 5% weaker in masstone. Colour is (DE=0.9 Mass) and (DE=1.1 Und). More economical product.
N/A | D-B601265 | [NAME] | 13 | N/A | N/A |  | 200 | Low | Non-FDA, [NAME] | Green | 6-8% | *DONOT USE*This is the color equivalent ot the B601260 275-0049. The 1231 is 5% weaker in masstone. Colour is (DE=1.4 Mass) and (DE=1.7 Und). More economical product.
N/A | D-B601266 | D-DCC 1202 Diarylide Yellow | PY 14 | N/A | N/A |  | 200 | low | Non FDA, [NAME] | green | 8 - 12 | *DONOT USE*
N/A | B601267 | [NAME] | N/A | N/A | N/A
268FE01 | B601268 | 6226 Synergy GR MS Yellow | NA | 0.01 | FCM | PG03638, PG07487/0108 / B4 | 300 | Medium | FDA | Red | 16 | Use [NAME] instead Zn-St in the formula. FDA compliant to maximum of 2% pigment in final product.
268FE10 | B601268 | Yellow 6226 |  | 0.1 | FCM | PG07487/0108 / B4
268HE01 | B601268 | 6226 Synergy GR MS Yellow |  | 0.01 | HIDM | B4
268FS05 | B601268 | 6226 Synergy GR MS Yellow |  | 0.05 | FCM | PG07487/B4
268HE10 | B601268 | 6226 Synergy GR MS Yellow |  | 0.1 | HIDM | B4
120LC005 | 120LC005 | Yellow 6226 Dryblend Intermediate |  | 0.05 | Powder Intermediate
269FE01 | B601269 | 6202 Synergy Yellow HG | N/A | 0.01 | FCM | PG03348, 10/2/06 / B5 | 300 | medium | FDA | green | 16 | Use [NAME] instead Zn-St. FDA compliant to maximum 1% in final part.
269FE10 | B601269 | 6202 Synergy Yellow HG |  | 0.1 | FCM | PG03348 / B5
269HE01 | B601269 | 6202 Synergy Yellow HG |  | 0.01 | HIDM | PG007725
269HE10 | B601269 | 6202 Synergy Yellow HG |  | 0.1 | HIDM | PG007725
120LC003 | 120LC003 | 6202 Synergy Yellow HG Dryblend Intermediate |  | 0.05 | Powder Intermediate
272HE50 | B601272 | [NAME]) | N/A | 0.5 | HIDM | B5 | 204 | high | [NAME] | green | 40 | For higher heat stable use [NAME] 17103
N/A | B601273 | [NAME] Resist LT Pale Gold | N/A | N/A | N/A
N/A | B601274 | L75-1349 Yellow 13(flush) | PY13 | N/A | N/A |  | 200 | Low | Non-FDA, [NAME] | medium-green-red | 30-40 | This is flush version of B601260 Yellow 275-0049. Pigment loading of this flush product is 50%. Use only when the maximum loading of the B601260/[NAME] is reached.Donot use for outdoor application.
N/A | B601275 | 1293 Rightfit Yellow | PY 212 | N/A | N/A |  | 316 | Poor | FDA, [NAME] | Red | 10-12 | FDA compliant to maximum of 1% in final product.
N/A | D-B601276 | D-I.O. Yellow 3020 | 12 | N/A | N/A |  | 220 | high | Non-FDA, [NAME] | dirty green | 40-42 | Utility [NAME]. Same as B601255 but less cost.
277FE01 | D-B601277 | D-PV Fast Yellow H9G | PY 214 | 0.01 | FCM | 10/2/06 / B5 | 280 | High | FDA, [NAME] | green | 10 - 12 | Slighly greener than B601230 KO961D; FDA compliant to maximum of 1% pigment in the final product.  Use ONLY IF B601230 is not available.
277HE10 | D-B601277 | D-YELLOW H9G |  | 0.1 | HIDM | B6
278FE01 | D-B601278 | D-1365 [NAME] | PY62 | 0.01 | FCM | B6 | 250 | Moderate | Non- FDA, [NAME] | Red | 12-16% | *DISCONTINUED DO NOT USE* USE B602216 INSTEAD
278FE10 | D-B601278 | D-1365 [NAME] |  | 0.1 | FCM | B6
278HE01 | D-B601278 | D-1365 [NAME] |  | 0.01 | HIDM | B6
278HE10 | D-B601278 | D-1365 [NAME] |  | 0.1 | HIDM | B6
281HE05 | D-B601281 | D-5020 Med Chrome Yelllow | PY34 | 0.05 | HIDM | B7 | 260 | high | Heavy metal, Lead based | red | 80% | **DISCONTINUED - DO NOT USE**  USE B602222  (Use for IM or higher heat application.  Always use Zn-St and B900 in formulations.)
281HE50 | D-B601281 | D-5020 Med Chrome Yelllow |  | 0.5 | HIDM | B7
282FE05 | D-B601282 | [NAME] [NAME] | PY34 | 0.05 | FCM | 10/2/06 / B7 | 260 | high | Heavy metal, Lead based | green | 80% | **DISCONTINUED** DO NOT USE; USE B602223 INSTEAD
282HE05 | D-B601282 | [NAME] [NAME] |  | 0.05 | HIDM
282HE50 | D-B601282 | [NAME] [NAME] |  | 0.5 | HIDM | B7
N/A | [NAME] | [NAME] | PY 110 | N/A | N/A |  | 300 | high | FDA, [NAME] | red | 10-12% | Use for high temperature outdoor application only
287HE10 | B601287 | US Made Yellow HGR |  | 0.1 | HIDM | B7
288HE10 | [NAME] | Iriodin 305 Solar Gold |  | 0.1 | HIDM | B7
289FE25 | D-B601289 | D-Iriodin 302 Satin Gold | Not Applicable | 0.25 | FCM |  | 600 | High | FDA | [NAME] | 20 - 25% | Particle size 5-25 microns. Fine brilliant gold w/ Anatase TiO2
289HE25 | D-B601289 | D-Iriodin 302 Satin Gold |  | 0.25 | HIDM | B8
290FE10 | B601290 | Iriodin 303 Royal Gold | Not Applicable | 0.1 | FCM | B8 | 600 | High | FDA | Royal Gold | 25% | Particle size 10-60 microns.Brilliant gold w/ Rutile TiO2
290HE10 | B601290 | Iriodin 303 Royal Gold |  | 0.1 | HIDM
N/A | D-B601291 | D-Iriodin  520 [NAME] | Not Applicable | N/A | N/A |  | 600 | High | FDA | [NAME] | 25 | Particle size 5-25 microns. Fine brilliant gold w/o TiO2
293HE10 | B601293 | Iriodin 363 Shimmer Gold | N/A | 0.1 | HIDM | B8 |  |  | FDA
293HE25 | B601293 | Iriodin 363 Shimmer Gold |  | 0.25 | HIDM | B8
294FE01 | B601294 | YELLOW IO. 4021 | PY 42 | 0.01 | FCM | 8/6/08 / B9 | 220 | HIGH | FDA | RED | 30-40% | DO NOT USE FOR IM OR BM APPLICATIONS. LOW COST IO YELLOW FOR BF APPLICATIONS. DO NOT USE FOR FORMULAS REQUIRING MI CARRIERS BELOW 20 MI
294FE10 | B601294 | YELLOW IO,4021 |  | 0.1 | FCM | 8/22/08 / B9
294FE20 | B601294 | YELLOW IO,4021 |  | 0.2 | FCM | 8/5/08 / B9
294HE20 | B601294 | YELLOW IO. 4021 |  | 0.2 | HIDM | B9
120LC006/02 | B601294 | Yellow Y-4021 Dryblend Intermediate |  | 0.05 | Powder Intermediate | 7/29/09
 | D-B601295 | D-MACROLEX YELLOW G |  | 1 |  |  | 300 | HIGH | FDA FOR PET, PS | GREEN | 0.1 | **DO NOT USE - DISCONTINUED**  USE B602229
120LC006 | 120LC006 | 5% DB YEL. Y4021 INTERM. | NA | 1 | DB
296FE01 | B601296 | [NAME] |  | 0.01 | FCM | Standard / B9 | 240 | HIGH | FDA | GREEN | 35-45% | REPLACES B601214 COLORTHERM 10.  HEAT STABLE IO YELLOW VERSION OF THE B601294
296FE25 | B601296 | [NAME] |  | 0.25 | FCM
120LC004 | 120LC004 | [NAME] Intermediate |  | 0.05 | Powder Intermediate | 3/20/07 / B10
299FE01 | D-B601299 | D-Bayferrox 420 | PY 42 | 0.01 | FCM |  | 220 | HIGH | FDA | RED | 30-40% | THIS PIGMENT IS DISCONTINUED AND ITS REPLACMENT IS B601294. THIS PIGMENT IS TO BE USED FOR UTILITY FILM APPLICATIONS. DO NOT USE FOR BM OR IM APPLICATIONS.
299HE01 | D-B601299 | D-Bayferrox 420 |  | 0.01 | HIDM | B10
299HE10 | D-B601299 | D-Bayferrox 420 |  | 0.1 | HIDM | B10
299HE50 | D-B601299 | D-Bayferrox 420 |  | 0.5 | HIDM | B10
299HV10 | D-B601299 | D-Bayferrox 420 |  | 0.1 | HIDM | 2716 S3
2211FE10 | B602211 | Yellow DCC 7180 | PY 180 | 0.1 | FCM | 2716 S3 | 280 | HIGH | FDA | MEDIUM GREEN | 8-12% | **DISCONTINUED**  DO NOT USE.  USE B602230.                                                                           HIGH LIGHFASTNESS BUT LIMITED WEATHERFASTNESS. FDA ACCEPTABLLE UP TO 1% PIGMENT IN FINAL PART
2211FE01 | B602211 | Yellow DCC 7180 |  | 0.01 | FCM | 2716 S3
2211HE10 | B602211 | Yellow DCC 7180 |  | 0.1 | HIDM | 2716 S3
2211HE01 | B602211 | Yellow DCC 7180 |  | 0.01 | HIDM | 2757 S1
2212FE10 | B602212 | Yellow DCC 7155 | PY 155 | 0.1 | FCM | 2757 S1 | 250 | LOW [NAME] | Non-FDA, [NAME] | GREEN | 10-12% | GOOD GREEN SHADE PIGMENT - LIMITED HEAT AND WEATHERFASTNESS STABILITY IN TINT APPLICATIONS.
2212FE01 | B602212 | Yellow DCC 7155 |  | 0.01 | FCM | 2757 S1
2212HE10 | B602212 | Yellow DCC 7155 |  | 0.1 | HIDM | 2757 S1
2212HE01 | B602212 | Yellow DCC 7155 |  | 0.01 | HIDM | 7142 S1
2213FE10 | B602213 | Yellow DCC 1368 | PY 168 | 0.1 | FCM | 7142 S1 | 250 | LOW [NAME] | HMF, NOT-FDA | GREEN | 10-12% | **TO BE USED ONLY IF B601237 [NAME] IS NOT AVAILABLE**
2213FE01 | B602213 | Yellow DCC 1368 |  | 0.01 | FCM | 7142 S1
2213HE10 | B602213 | Yellow DCC 1368 |  | 0.1 | HIDM | [NAME]
2213HE01 | B602213 | Yellow DCC 1368 |  | 0.01 | HIDM | Master [NAME]
2214HE10 | B602214 | [NAME] |  | 0.1 | HIDM | 2-0909-0764/1009
2214HE25 | B602214 | [NAME] |  | 0.25 | HIDM | 2-0909-0764/1009
2214FE10 | B602214 | [NAME] |  | 0.1 | FCM | 2-0909-0764/1009
2214FE25 | B602214 | [NAME] |  | 0.25 | FCM | 2-0909-0764/1009
2215FE25 | B602215 | Yellow-Orange BNF-OY516 |  | 0.25 | FCM
2215FE10 | B602215 | Yellow-Orange BNF-OY516 |  | 0.1 | FCM
2215FE01 | B602215 | Yellow-Orange BNF-OY516 |  | 0.01 | FCM
2216FE10 | B602216 | Sun 262-3562 | PY 62 | 0.1 | FCM | Master [NAME] | 240 | LOW [NAME] | HMF, NOT-FDA | RED | 12-15% | THIS PIGMENT REPLACES B601239 YELLOW WSR
2216FE01 | B602216 | Sun 262-3562 |  | 0.01 | FCM
2216HE10 | B602216 | Sun 262-3562 |  | 0.1 | HIDM
2216HE01 | B602216 | Sun 262-3562 |  | 0.01 | HIDM
2217FE10 | B602217 | Sun 275-9849 (PY13) | PY 13 | 0.1 | FCM | Master [NAME] | 200 | LOW | HMF, NOT FDA, DIARYLIDE | Mid Green-Red | 8-10% | NOT TO BE USED FOR TMEPREATURES ABOVE 200C - 400F - USE ZnSt AT 1.5% FOR AMOUNTS GREATER THAN 8% IF CUSTOMER APPLICATION ALLOWS IT. DO NOT USE IN INJECTION MOLDING APPLICATIONS
2217FE01 | B602217 | Sun 275-9849 (PY13) |  | 0.01 | FCM
2217HE10 | B602217 | Sun 275-9849 (PY13) |  | 0.1 | HIDM
2217HE01 | B602217 | Sun 275-9849 (PY13) |  | 0.01 | HIDM
2218FE10 | B602218 | L69-4534 FD&C Yellow No. 5 |  | 0.1 | FCM | CIBK027B/1009 | 240 | LOW | FDA | RED | 20-25% | **THIS IS A FLUSH VERSION OF B601250**
2218FE01 | B602218 | L69-4534 FD&C Yellow No. 5 |  | 0.01 | FCM | CIBK027B/1009
2218HE10 | B602218 | L69-4534 FD&C Yellow No. 5 |  | 0.1 | HIDM | CIBK027B/1009
2218HE01 | B602218 | L69-4534 FD&C Yellow No. 5 |  | 0.01 | HIDM | CIBK027B/1009
2219HE50 | B602219 | [NAME] | PY 34 | 0.5 | HIDM | Master [NAME] | 240 | HIGH | LEAD BASED | RED | 0.5 | **DO NOT USE for Injection Molding or High Heat Application** For IM, use  B602222 instead. Always use Zn St & B900 in the formula.
2219HE10 | B602219 | [NAME] |  | 0.1 | HIDM | Master [NAME]
2219HE01 | B602219 | [NAME] |  | 0.01 | HIDM | Master [NAME]
2220HE50 | B602220 | [NAME] | PY 34 | 0.5 | HIDM | Master [NAME] | 240 | HIGH | LEAD BASED | GREEN | 0.5 | **DO NOT USE for Injection Molding or High Heat Application** For IM, use  B602223 instead. Always use Zn St & B900 in the formula
2220HE10 | B602220 | [NAME] |  | 0.1 | HIDM | Master [NAME]
2220HE01 | B602220 | [NAME] |  | 0.01 | HIDM | B12
2221HE50 | B602221 | [NAME] | PY 34 | 0.5 | HIDM |  | 250 | medium | Hemay Metal, Lead Chromate | Green | 60% | MUST USE ZnSt AND A/O TO MAINTAIN COLOUR SHADE
2221HE10 | B602221 | [NAME] |  | 0.1 | HIDM
2221HE01 | B602221 | [NAME] |  | 0.01 | HIDM
2222HE50 | B602222 | [NAME] | PY 34 | 0.5 | HIDM |  | 260 | HIGH | Hemay Metal, Lead Chromate | RED | 0.6 | MUST USE ZnSt AND A/O TO MAINTAIN COLOUR SHADE
2222HE10 | B602222 | [NAME] |  | 0.1 | HIDM
2222HE01 | B602222 | [NAME] |  | 0.01 | HIDM
2223FE50 | B602223 | [NAME] | PY 34 | 0.5 | FCM |  | 260 | high | Heavy metal, Lead based | green | 80% | Use for IM or higher heat application.  Always use Zn-St and B900 in formulations.
2223FE10 | B602223 | [NAME] |  | 0.1 | FCM
2223FE01 | B602223 | [NAME] |  | 0.01 | FCM
2224HE10 | D-B602224 | Yellow 275-4570 (PY 83) | PY 83 | 0.1 | HIDM |  | 200 | LOW | [NAME] | RED | 8-10% | NOT TO BE USED FOR TMEPREATURES ABOVE 200C - 400F - USE ZnSt AT 1.5% FOR AMOUNTS GREATER THAN 8% IF CUSTOMER APPLICATION ALLOWS IT. DO NOT USE IN INJECTION MOLDING APPLICATIONS
2224HE01 | D-B602224 | Yellow 275-4570 (PY 83) |  | 0.01 | HIDM
2224FE10 | D-B602224 | Yellow 275-4570 (PY 83) |  | 0.1 | FCM
2224FE01 | D-B602224 | Yellow 275-4570 (PY 83) |  | 0.01 | FCM
2225HE10 | B602225 | 274-5126 Sunbrite Yellow 14 | PY 14 | 0.1 | HIDM | 29096512/1009 | 200 | LOW | [NAME] | GREEN | 8-10% | NOT TO BE USED FOR TMEPREATURES ABOVE 200C - 400F - USE ZnSt AT 1.5% FOR AMOUNTS GREATER THAN 8% IF CUSTOMER APPLICATION ALLOWS IT. DO NOT USE IN INJECTION MOLDING APPLICATIONS
2225HE01 | B602225 | 274-5126 Sunbrite Yellow 14 |  | 0.01 | HIDM | 29096512/1009
2225FE10 | B602225 | 274-5126 Sunbrite Yellow 14 |  | 0.1 | FCM | 29096512/1009
2225FE01 | B602225 | 274-5126 Sunbrite Yellow 14 |  | 0.01 | FCM | 29096512/1009
2227FE25 | D-B602227 | D-Meteor Yellow [NAME] 9379 | PBr 24 | 0.25 | FCM |  | 320 | HIGH | [NAME] | RED | 30-40% | **DO NOT USE. DISCONTINUED. USE B601254 INSTEAD.**       Weak, inorganic FDA yellow. Use only when [NAME] or Yellow Y-905K  cannot be used due to tempertaure limitations.  '*FDA Compliant to maximum of 2% pigment in final product.*
2227FE10 | D-B602227 | D-Meteor Yellow [NAME] 9379 | PBr 24 | 0.1 | FCM
2227FE01 | D-B602227 | D-Meteor Yellow [NAME] 9379 | PBr 24 | 0.01 | FCM
120LC008 | D-120LC008 | D- [NAME] 9379 Dryblend  Intermediate |  | 0.05 | Powder Intermediate
2230FE10 | B602230 | Verdcol BML Yellow 180 2T |  | 0.1 | FCM | 91018
2230FE01 | B602230 | Verdcol BML Yellow 180 2T |  | 0.01 | FCM
2230HE10 | B602230 | Verdcol BML Yellow 180 2T |  | 0.1 | HIDM
2230HE01 | B602230 | Verdcol BML Yellow 180 2T |  | 0.01 | HIDM
2229FS05 | B602229 | Keystone Yellow AG |  | 0.05 | FCM |  | 280-300 depending on host resin | High | FDA for PET only
XMICA-6300HE25 | [NAME] | Sun Mica 284-6300 Gold |  | 0.25 | HIDM
XYEL-RNHE10 | XYEL-RN | [NAME] |  | 0.1 | HIDM | CHS23592 / B12
300FE01 | B601300 | 6113 Synergy Orange |  | 0.01 | FCM | PG04845/ B12
300FE10 |  | 6113 Synergy Orange |  | 0.1 | FCM
308HE10 | B601308 | ZQ-15 Blaze Orange | NA | 0.1 | HIDM |  | 300 | Poor | Non-FDA, [NAME] | Red | 30-40% | Do not use [NAME] or CaSt in combination with this pigment. Melting point of the polyamide carrier resin is 175C, We must meet Melting point in order to develop the color.
308HE25 | B601308 | ZQ-15 Blaze Orange |  | 0.25 | HIDM
308HV10 | B601308 | ZQ-15 Blaze Orange |  | 0.1 | HIDM | B13
308HV25 | B601308 | ZQ-15 Blaze Orange |  | 0.25 | HIDM | B13
309HE10 | D-B601309 | D-ZQ-14 Fire Orange | NA | 0.1 | HIDM |  | 300 | Poor | Non-FDA, [NAME] | Red | 30-40% | **DO NOT USE - DISCONTINUED**  USE B601316                                             Do not use [NAME] or CaSt in combination with this pigment. Melting point of the polyamide carrier resin is 175C, We must meet Melting point in order to develop the color.
309HE25 | D-B601309 | D-ZQ-14 Fire Orange |  | 0.25 | HIDM
309HV10 | D-B601309 | D-ZQ-14 Fire Orange |  | 0.1 | HIDM | B14
309HV25 | D-B601309 | D-ZQ-14 Fire Orange |  | 0.25 | HIDM | B14
N/A | B601310 | Microlen DPP Orange TR-MC | P.O. 71 | N/A | N/A |  | 300 | high | FDA, [NAME] | red | 20-25% | Predispersed product with 50% pigment loading of B601311. For use in Clarified FDA PP application.
N/A | B601311 | Cromophtal DPP Orange TR | PO 71 | N/A | N/A |  | 300 | high | FDA, [NAME] | red | 10-12% | For use in Clarified FDA PP application.
312FE01 | [NAME] | GP Cromophtal Orange | 64 | 0.01 | FCM | B14 | 270 | high | FDA | Blue | 10 - 15% | FDA compliant. Use when clean orange look required and high light fastness required.
312FE10 | [NAME] | GP Cromophtal Orange |  | 0.1 | FCM | B15
312HE10 | [NAME] | GP Cromophtal Orange |  | 0.1 | HIDM | 01253BJ7 / B15
313FE01 | B601313 | Engeltone 2920 Orange | PO79 | 0.01 | FCM | Jan./06 / B15 | 280 | low | FDA, [NAME] | Yellow | 10-12% | Use instead of Orange GP B601312.* FDA compliant to maximum of 1% pigment in final product.
313FE10 | B601313 | Engeltone 2920 Orange |  | 0.1 | FCM
313HE10 | B601313 | Engeltone 2920 Orange |  | 0.1 | HIDM
313FS05 | B601313 | Engeltone 2920 Orange |  | 0.05 | FCM | PG08334/B15
13901C18 | 13901C18 | Orange 2920 Dryblend |  | 0.05 | Powder Intermediate
314HS01 | D-B601314 | [NAME] ORANGE 3G |  | 0.01 | HIDM | B16 |  |  |  |  |  | **DISCONTINUED** USE B601317 INSTEAD
316HE25 | B601316 | BNF-OR514 ORANGE-RED FLUORESCENT |  | 0.25 | HIDM | 902-0460-0609
316HE10 | B601316 | BNF-OR514 ORANGE-RED FLUORESCENT |  | 0.1 | HIDM | 902-0460-0609
317FS05 | B601317 | Buckeye Orange LFP |  | 0.05 | FCM | 080416/0909
321FS05 | B601321 | Keyplast Orange MR |  | 0.05 | FCM | A209I278 | 280-300 depending on host resin | Good to High; dependin on host resin | FDA for PS & PET
330HE10 | B601330 | 276-2384 Sunbrite Orange 13 | PO 13 | 0.1 | HIDM | B16 | 180 | Poor | Non-FDA, [NAME] | Red | 6-8% | DO NOT USE THIS PIGMENT UNLESS SPECIFIED IN LRN - NOT HEAT STABLE
338FE50 | B601338 | Orange NM-33 | R104 | 0.5 | FCM | 09/29/08
338FE10 | B601338 | Orange NM-33 |  | 0.1 | FCM | 09/29/08
130LC004 | 130LC004 | Orange NM-33 Dryblend Intermediate |  | 0.05 | Powder Intermediate
339FE50 | B601339 | Orange NL-39 | R104 | 0.5 | FCM | 11/12/08
339FE10 | B601339 | Orange NL-39 |  | 0.1 | FCM | 11/12/08
341HE10 | D-B601341 | D-1623 Moly Orange (Pb) | R104 | 0.1 | HIDM | 14592 / B16 | 240 | Good(1 year [NAME]) | Heavy Metal Base (Lead) | Yellow | 80 | Yellowest shade. Always use [NAME] and B900 in formula *DISCONTINUED USE B601338 INSTEAD*
341HE50 | D-B601341 | D-1623 Moly Orange (Pb) |  | 0.5 | HIDM | 22760 / B16
342HE10 | D-B601342 | D-1610/2517 Moly Orange (Pb) | R-104 | 0.1 | HIDM | 21518 / B16 | 260 | high | Heavy Metal Based (Lead) | Yellow | 80 | Predarkened  yellow shade. Always use [NAME] and B900 in formula *DISCONTINUED DO NOT USE* USE B601338 INSTEAD
342HE50 | D-B601342 | D-1610/2517 Moly Orange (Pb) |  | 0.5 | HIDM | 21518 / B17
343HE10 | D-B601343 | D-1606 Moly Orange (Pb) | R-104 | 0.1 | HIDM | B17 | 260 | high | Heavy Metal Based (Lead) | Blue | 80 | Predarkened red shade. Always use [NAME] and B900 in formula *DISCONTINUED DO NOT USE* USE B601339 INSTEAD
344HE10 | D-B601344 | [NAME] (Pb) | R-104 | 0.1 | HIDM | B17 | 260 | good (1 year [NAME]) | Heavy  Metal Based (Lead) | Blue | 80 | Predarkened bluest shade. Always use [NAME] and B900 in formula *DISCONTINUED DO NOT USE* USE B601339 INSTEAD
N/A | B601345 | KO-906 [NAME] | R104 | N/A | N/A |  | 300 | High | Heavy Metal, Lead | Blue | 80 | Heat stable pigment, similar in shade as the 1610 but 30% weaker due to the silica coating on the KO906 pigment. PROBLEMS WITH MOISTURE.
N/A | B601346 | KY-909 [NAME] | R104 | N/A | N/A |  | 300 | Good | Heavy Metal, Lead | Yellow | 40-50 | Heat stable pigment, similar in shade as the 1624 but 30% weaker due to the silica coating on the [NAME] pigment. PROBLEMS WITH MOISTURE. USE WITH CARE
N/A | D-B601347 | D-2-5 Ming Orange Medium (Pb) | R-104 | N/A | N/A |  | 260 | High | Heavy Metal Based (Lead) | Yellod | 45 - 50% | *DISCONTINUED DONOT USE*  Close to 1610. Always use [NAME] and B900 in formula.
N/A | D-B601348 | D-2517 Moly Orange (Pb) | R-104 | N/A | N/A |  | 260 | High | Heavy Metal Based (Lead) | Yellow | 45 - 50% | *DISCONTINUED DONOT USE* Alternate to 1610. Always use [NAME] and B900 in formula.
349HE01 | D-B601349 | D-5610 Moly Orange | R104 | 0.01 | HIDM | 14253 / B17 | 280 | high | Heavy metal, Lead based | yellow | 80 | **DISCONTINUED; DO NOT USE** USE B601353                                       Use for IM application or higher heat application Always use Zn-st & B900 in formula
349HE10 | D-B601349 | D-5610 Moly Orange |  | 0.1 | HIDM | B17
350HE01 | D-B601350 | D-5606 Moly Orange | N/A | 0.01 | HIDM | B17 | 280 | high | Heavy metal, Lead based | blue | 80 | **DISCONTINUED;  DO NOT USE** USE B601352                             Use for IM or higher heat application Always use Zn-St & B-900 in formula
350HE10 | D-B601350 | D-5606 Moly Orange |  | 0.1 | HIDM | B18
352HE50 | B601352 | Nubiola NRC-36 Moly Orange | R104 | 0.5 | HIDM | B19 | 260 | high | Heavy metal, Lead based | BLUE | 0.7 | ALWAYS USE ZnSt AND B900 IN FORMULA
352HE10 | B601352 | Nubiola NRC-36 Moly Orange |  | 0.1 | HIDM
352HE01 | B601352 | Nubiola NRC-36 Moly Orange |  | 0.01 | HIDM
353HE50 | B601353 | Nubiola NR-38 Moly Orange | R104 | 0.5 | HIDM |  | 260 | high | Heavy metal, Lead based | YELLOW | 0.7 | ALWAYS USE ZnSt AND B900 IN FORMULA
353HE10 | B601353 | Nubiola NR-38 Moly Orange |  | 0.1 | HIDM
353HE01 | B601353 | Nubiola NR-38 Moly Orange |  | 0.01 | HIDM
XORA-RFS01 | Xora-R | [NAME] R |  | 0.01 | FCM
400HE01 | D-B601400 | D-RO-3097 Iron Oxide Red | R-101 | 0.01 | HIDM | [NAME] | 600 | Very High | FDA | Yellow | 45 - 50% | *Use B601472 Red 120 NM instead* High heat and lightfastness stability. Not micronized
400HE10 | D-B601400 | D-RO-3097 Iron Oxide Red |  | 0.1 | HIDM | 2016J001056/0308 / B20
400HE20 | D-B601400 | D-RO-3097 Iron Oxide Red |  | 0.2 | HIDM | [NAME]
401FE01 | D-B601401 | D-RO-8097 Iron Oxide  Red | R-101 | 0.01 | FCM |  | 600 | Very High | FDA | Blue | 45 - 50% | High heat and lightfastness stability. Not micronized *USE B601473 INSTEAD*
401FE20 | D-B601401 | D-RO-8097 Iron Oxide  Red |  | 0.2 | FCM
401HE01 | D-B601401 | D-RO-8097 Iron Oxide  Red |  | 0.01 | HIDM
401HE05 | D-B601401 | D-RO-8097 Iron Oxide  Red |  | 0.05 | HIDM
401HE20 | D-B601401 | D-RO-8097 Iron Oxide  Red |  | 0.2 | HIDM
401HS10 | D-B601401 | D-RO-8097 Iron Oxide  Red |  | 0.1 | HIDM | 65010010 / B20
14907C18 | D-14907C18 | D-RED 8097 DRY BLEND | NA | 0.05 | Powder Intermediate |  | 600 | Very High | FDA | Blue | 45-50% | 'High heat and lightfastness stability. Not micronized
N/A | D-B601402 | D-Red 9998 Iron Oxide | R101 | N/A | N/A |  | 1000 | High | FDA, [NAME] | Blue | 40-50% | This pigment is much bluer and darker than the Red 8097. Use only when absolutly necessary.
406HM10 | D-B601406 | D-ZQ-12 Neon Red | N/A | 0.1 | HIDM | T04May14 / B20 | 300 | Poor | Non-FDA, [NAME] | Blue | 15-25% | **DISCONTINUED - DO NOT USE**  USE B601488
407FE10 | B601407 | L15-1210 Red Lake C (flush) | 53:1 | 0.1 | FCM | D37406 / [NAME] | 260 | Extremelly Poor | Non-FDA, [NAME] | Yellow Shade | 20-30% | Predispersed pigment. [NAME] release. Similar to 2509 Red Lake
407HE10 | B601407 | L15-1210 Red Lake C (flush) |  | 0.1 | HIDM
408FE01 | D-B601408 | D-2509C Red Lake C | 53:1 | 0.01 | FCM | 6/27/06 / B21 | 280 | Extremelly Poor | Non-FDA, [NAME] | Yellow | 10-12% | *Use B601477Red LG instead*  Use B601407 to maximize loading.[NAME] release
408FE10 | D-B601408 | D-2509C Red Lake C |  | 0.1 | FCM | B21
408HE10 | D-B601408 | D-2509C Red Lake C |  | 0.1 | HIDM | B21
N/A | D-B601410 | D-3RLP Graphtol Rubine Red | 48:3 | N/A | N/A |  | 240 | Moderate | Non-FDA, [NAME] | Blue | 8 - 12% | Do not use - Expensive version of 4BP and L4BD red from CIBA
N/A | D-B601411 | D-RV-6832 Magenta | 122 | N/A | N/A |  | 280 | Excellent | [NAME] | Blue | 8 - 12% | DISCONTINUED. Use Red ERV-8655 - It's stronger & softer
N/A | D-B601412 | D-WTP Graphtol Rubine Red | 48:2 | N/A | N/A |  | 260 | Moderate | Non-FDA, [NAME] | Blue | 8 - 12% | *DONOT USE*  Similar to 6197 red from Bayer & 2BP from Ciba
N/A | D-B601413 | D-L4BD Irgalite Rubine Red | 57:1 | N/A | N/A |  | 240 | Moderate | Non-FDA, [NAME] | Blue | 7 - 10% | *DONOT USE* Similar to 4BP red, but more difficult to disperse
N/A | D-B601414 | D-R-6704 Quindo Red | Violet 19 | N/A | N/A |  | 280 | Excellent | [NAME] | Blue | 7 - 10% | *DONOT USE*
N/A | D-B601415 | D-PV Fast Red BNP | 214 | N/A | N/A |  | 280 | Really Good | Non-FDA, [NAME] | Blue | 8 - 12% | High lightfastness. Good for outdoor application
N/A | D-B601416 | D-PVFR HF4B Red | 187 | N/A | N/A |  | 250 | Excellent | [NAME] | Blue | 8 - 12% | Not often used. Dirty tone. Ideal for FDA & outdoor application
N/A | D-B601417 | D-PV Fast Red B | 149 | N/A | N/A |  | 300 | Excellent | Non-FDA, [NAME] | Yellow | 8 - 12% | Not often used. For outdoor application. Causes warping  in HDPE
N/A | D-B601418 | D-C19-6627  FD&C Red | FD&C Red #7 | N/A | N/A |  | 230 | Poor | [NAME] | Blue | 6 - 10% | DISCONTINUED. Use pigment C19-003->weaker but same shade
419FE01 | D-B601419 | D-Bayplast Red 2B (Powder) | 48:2 | 0.01 | FCM | 6/27/06 / B21 | 240 | Moderate | Non-FDA, [NAME] | Medium Blue | 8 - 12% | *Use B601458 Red BBC instead* Not as blue as 4BP/L4BD. Similar to Red 2BP from Ciba
419FE10 | D-B601419 | D-Bayplast Red 2B (Powder) |  | 0.1 | FCM
419HE10 | D-B601419 | D-Bayplast Red 2B (Powder) |  | 0.1 | HIDM | B21
422FE10 | D-B601422 | D-C19-003 FD&C Red #7 Ca Lake | FD&C Red #7 | 0.1 | FCM | 584213 / B21 | 230 | Poor | [NAME] | Blue | 6 - 10% | Low bulk density. Watch for maximum loading. [NAME] release
N/A | B601423 | D-Microlen Red 2BSP (Flush) | 48:3 | N/A | N/A |  | 240 | Moderate | Non-FDA, [NAME] | Yellow | 20 - 30% | Predispersed version of Red 2BSP Irgalite Red  (50% pigment)
424FE01 | [NAME] | 2BSP Irgalite Red | 48:3 | 0.01 | FCM | 90603FW3 / B22 | 250 | Moderate | Non-FDA, [NAME] | Yellow | 8 - 12% | Bluer than 2BY red but yellower than 4BP/L4BD; **USE B601492 SUN 234-7483 AS AN ALTERNATE PIGMENT**
424FE10 | [NAME] | 2BSP Irgalite Red |  | 0.1 | FCM
424FV10 | [NAME] | 2BSP Irgalite Red |  | 0.1 | FCM | 60091FW6 / B22
424FS01 | [NAME] | 2BSP Irgalite Red |  | 0.01 | FCM
424HS01 | [NAME] | 2BSP Irgalite Red |  | 0.01 | HIDM | B22
425FE01 | D-B601425 | D-2BY Irgalite Red | 48:3 | 0.01 | FCM | Jan./06 / B22 | 240 | Moderate (6 months) | Non-FDA, [NAME] | Yellow | 8-10% | *Use Red B601457 Red GG* Yellowest of all reds. Strantium Base
425FE10 | D-B601425 | D-2BY Irgalite Red |  | 0.1 | FCM | B23
N/A | D-B601426 | D-BP Chromophtal DPP Red | 254 | N/A | N/A |  | 300 | High | FDA, [NAME] | Medium Blue shade | 10-12% | Expensive FDA Red. Use for FDA or for high lightfast outdoor application. Tends to warp
427FE01 | B601427 | 4BP Irgalite Rubine Red | 57:1 | 0.01 | FCM | 900427 U9 V1, Jan./06 / B23 | 240 | Moderate (6 months) | Non-FDA, [NAME] | Blue | 7-9% | Bluest shade in all reds. Similar in color to L4BD, but with better dispersion characteristics
427FE10 | B601427 | 4BP Irgalite Rubine Red |  | 0.1 | FCM | B23
427FE14 | B601427 | 4BP Irgalite Rubine Red |  | 0.14 | FCM | 60038FW7 / B23
427FM10 | B601427 | 4BP Irgalite Rubine Red |  | 0.1 | FCM | 60038FW7 / B24
427HE01 | B601427 | 4BP Irgalite Rubine Red |  | 0.01 | HIDM | 60038FW7 / B23
427HE10 | B601427 | 4BP Irgalite Rubine Red |  | 0.1 | HIDM
427HS01 | B601427 | 4BP Irgalite Rubine Red |  | 0.01 | HIDM | B24
14902C18 | 14902C18 | 4BP Irgalite Rubine Red Dryblend Intermediate |  | 0.05 | Powder Intermediate
N/A | D-B601428 | D-Microlen 2BP Red (Flush) | 48:2 | N/A | N/A |  | 230 | Moderate (6 months) | Non-FDA, [NAME] | Medium Blue | 8-10% | Flush pigment (50%). Only use when dispersion is bad. DO NOT USE. USE B601431
429HE10 | B601429 | Microlen 4BP Red (Flush) | 57:1 | 0.1 | HIDM | B24 | 240 | Moderate (6 months) | Non-FDA, [NAME] | Blue | Up to 20% | Predispersed version of B601427 Irgalite 4BP. Use only when dispersion is bad
431FE10 | D-B601431 | D-L34-1209 2B Red (Flush) | 48:2 | 0.1 | FCM | DC3411 / B24 | 230 | Moderate (6 months) | Non-FDA, [NAME] | Medium Blue | Up to 20% | **DISCONTINUED** DO NOT USE - USE B601478                                                Flush Pigment (50%) similar to Microlen 2BP. Use this pigment instead of 2BP
431HE10 | D-B601431 | D-L34-1209 2B Red (Flush) |  | 0.1 | HIDM | DA2412 / B24
432FE01 | D-B601432 | D-Bayferrox 110 Red Iron Oxide | Red 101 | 0.01 | FCM | Jan./06 / B24 | 1000 | High | FDA, [NAME] | Yellow | 50% | Yellowest Iron Oxide red. High heat stability and lightfastness *DISCONTINUED DO NOT USE* USE B601472 INSTEAD
432FE20 | D-B601432 | D-Bayferrox 110 Red Iron Oxide |  | 0.2 | FCM
432HE01 | D-B601432 | D-Bayferrox 110 Red Iron Oxide |  | 0.01 | HIDM
432HE10 | D-B601432 | D-Bayferrox 110 Red Iron Oxide |  | 0.1 | HIDM | CH7100724 / C1
432HE20 | D-B601432 | D-Bayferrox 110 Red Iron Oxide |  | 0.2 | HIDM | C1
432HM01 | D-B601432 | D-Bayferrox 110 Red Iron Oxide |  | 0.01 | HIDM | CH7082746 / C1
14906C18 | D-14906C18 | D-RED 110 DRY BLEND | NA | 0.05 | Powder Intermediate |  | 100 | High | FDA, [NAME] | Yellow | 0.5 | 'Yellowest Iron Oxide red. High heat stability and lightfastness
433HE01 | D-B601433 | D-Bayferrox 120NM Red Iron Oxide | R-101 | 0.01 | HIDM | CH7080757 / C2 | 1000 | High | FDA, [NAME] | Medium Yellow | 50% | Bluer than Bayferrox Red 110, but yellower than Red 8097 *USE B601472 INSTEAD*
433HE10 | D-B601433 | D-Bayferrox 120NM Red Iron Oxide |  | 0.1 | HIDM | CH7080757 / C1
434FE01 | D-B601434 | D-'Graphtol Red LG Lake C | PR 53:1 | 0.01 | FCM | 6/27/06 / C2 | 270 | poor | Non FDA, [NAME] | Yellow | 10-12% | **DISCONTINUED - USE B601477 ** 'Same color as B601408 but 30% stronger and less cost.
434FE10 | D-B601434 | D-'Graphtol Red LG Lake C |  | 0.1 | FCM | 500788 / C2
434HE10 | D-B601434 | D-'Graphtol Red LG Lake C |  | 0.1 | HIDM | M STD, 4/25/08 / C2
N/A | B601436 | FD&C Red Lake 40 | N/A | N/A | N/A | N/A |  |  |  |  |  | **DO NOT USE FOR COLOUR MATCHING - USED AS A CUSTOKER REQUESTED PIGMENT FOR TOOTHPASTE APPLICATION**
N/A | D-B601438 | D-Irgazin DPP Red BO | 254 | N/A | N/A |  | 300 | High | FDA, [NAME] | Medium Blue | 8-10% | *DONOT USE* Use B601449 intead. Similar to DPP red BP, but good for applications when low warping is required
439FE01 | [NAME] | Rightfit Red K4350 | PR 277 | 0.01 | FCM | PG08084 / C2 | 288 | medium | FDA, [NAME] | Medium yellow-blue | 10-12% | *FDA Compliant to maximum of 2% pigment in final product
439FE10 | [NAME] | Rightfit Red K4350 |  | 0.1 | FCM | PG08084 / C3
439HE01 | [NAME] | Rightfit Red K4350 |  | 0.01 | HIDM
439HE10 | [NAME] | Rightfit Red K4350 |  | 0.1 | HIDM | PG08084,PG06034 / C3
140LC012 | 140LC012 | Rightfit Red K4350 Dryblend Intermediate |  | 0.05 | Powder Intermediate |  | 240 | MEDIUM | FDA,[NAME] | MEDIUM YELLLOW-BLUE | 0.05
440FE01 | B601440 | Rightfit Red K3790 | PR 276 | 0.01 | FCM | PG06029,PG00687 / C4 | 288 | medium | FDA, [NAME] | yellow | 10-12% | *FDA Compliant to maximum of 2% pigment in final product
440FE10 | B601440 | Rightfit Red K3790 |  | 0.1 | FCM | PG06029 / C4
440HE01 | B601440 | Rightfit Red K3790 |  | 0.01 | HIDM | PG07955 / C4
440HE10 | B601440 | Rightfit Red K3790 |  | 0.1 | HIDM
140LC017 | B601440 | Rightfit Red K3790 |  | 0.05 | Powder Intermediate
441FE10 | B601441 | 6012 Syenergy Red |  | 0.1 | FCM
442HE25 | D-B601442 | D-Iriodin 504 Red | Not Applicable | 0.25 | HIDM | 0504220 / C5 | 300 | High | FDA, [NAME] | Red | 25% | **DISCONTINUED** DO NOT USE.  USE B601494 INSTEAD.
443HE10 | B601443 | Chromophtal RED 2028 | 254 | 0.1 | HIDM | STD / C5 | 300 | High | FDA, [NAME] | YELLOW | 10-12% | Use this pigment for non-warping applications where the Red 2030 can not be used
443HE01 | B601443 | Chromophtal Red 2028 |  | 0.01 | HIDM | 00285HH9
443HE10 | B601443 | Chromophtal Red 2028 |  | 0.1 | HIDM | 00285HH9
443FE01 | B601443 | Chromophtal Red 2028 |  | 0.01 | FCM | 00285HH9
443FE10 | B601443 | Chromophtal Red 2028 |  | 0.1 | FCM | 00285HH9
444FE10 | D-B601444 | D-Microlen Red 2030-MC Flush |  | 0.1 | FCM | 175702M2 / C5 | 300 | High
446FE05 | B601446 | C19-011 D&C RED #7 CA LAKE |  | 0.05 | FCM | AMD80195 |  |  |  |  |  | USE AS AN ALTERNATE TO B601467
448FE01 | B601448 | Cromophtal Red 2020 | V19 | 0.01 | FCM | 02859HH8, C5
448FE10 | B601448 | Cromophtal Red 2020 |  | 0.1 | FCM | 02859HH8, C5 | 300 | High | FDA, [NAME] | Blue | 8-12%
448FS05 | B601448 | Cromophtal Red 2020 |  | 0.05 | FCM | 02859HH8, [NAME]
448HE10 | B601448 | Cromophtal Red 2020 |  | 0.1 | HIDM | C5
140LC014 | B601448 | Red 2020 Dryblend Intermediate |  | 0.05 | Powder Intermediate
449FE01 | B601449 | Sun 226-5254/Red 2030(CIBA) | 254 | 0.01 | FCM | 1901670AA, 6/27/06 / C6
449FE10 | B601449 | Sun 226-5254/Red 2030(CIBA) |  | 0.1 | FCM | C6 | 300 | High | FDA, [NAME] | Yellow | 10-12% | *FDA compliant to maximum of 1.0% of pigment in final product* Use instead of the B601426 Red DPP BP. Almost the same shade (yellower) and equivalent opacity. Use for FDA and high perfromance red applications. For IM application add 10-20% of B800501 [NAME] depend on the amount of this pigment in the formula to prevent warping.
449HE01 | B601449 | Sun 226-5254/Red 2030(CIBA) |  | 0.01 | HIDM | 20384HH7 / C6
449HE10 | B601449 | Sun 226-5254/Red 2030(CIBA) |  | 0.1 | HIDM
449FS10 | B601449 | Sun 226-5254/Red 2030(CIBA) |  | 0.1 | FCM | C7
449HMO1 | B601449 | Sun 226-5254/Red 2030(CIBA) |  | 0.01 | HIDM | 0691HH6 / C7
14909C18 | 14909C18 | Sun 226-5254/Red 2030(CIBA) Intermediate |  | 0.05 | Powder Intermediate
450FE01 | B601450 | 228-6655 Magenta B | 122 | 0.01 | FCM | G34Q05, Jan./06 / C8 | 300 | High | FDA, [NAME] | Medium Blue/Magenta | 10-12% | *FDA compliant to maximum of 1% of pigment in final product* Strong magenta . Bluer than 8672 but yellower than 8654
450FE10 | B601450 | 228-6655 Magenta B |  | 0.1 | FCM | G34Q05,83120-001, G77Q79 / C7
450FS10 | B601450 | 228-6655 Magenta B |  | 0.1 | FCM | GA6Q25 / C8
450HE01 | B601450 | 228-6655 Magenta B |  | 0.01 | HIDM | G37Q75 / C8
450HE10 | B601450 | 228-6655 Magenta B |  | 0.1 | HIDM
450HS10 | B601450 | 228-6655 Magenta B |  | 0.1 | HIDM
450HM01 | B601450 | 228-6655 Magenta B |  | 0.01 | HIDM | G86Q89 / C9
15901C18 | 15901C18 | MAGENTA 228-6655 DRY BLEND |  | 0.05 | Powder Intermediate
451HE10 | B601451 | 228-8653 Violet R | V19 | 0.1 | HIDM | C9 | 300 | High | FDA, [NAME] | Blue | 10-12% | Strong violet, FDA compliant. Bluer than 8655
N/A | D-B601452 | D-228-8672 Red 4B (Powder) | V19 | N/A | N/A |  | 300 | High | FDA, [NAME] | Yellow | 10-12% | *Discontinued pigment use red 2020 B601448 instead.*Strong violet, FDA compliant. Yellower than 8655 and 8654.
454FE036 | D-B601454 | D-PV Fast Pink E-01 | PR 122 | 0.036 | FCM | C9 | 300 | high | FDA, [NAME] | blue | 10-12% | *Use only for Kodak*   FDA compliant up to 1% in final product          454FE036 AKA: 14914-08 Red Intermediate for 11622-08
455FE01 | B601455 | 228-8673 Sunplast Red | PV 19 | 0.01 | FCM | BP40575 / C9 | 300 | High | FDA, [NAME] | Blue | 10-12% | Low dust granular pigment. Bluer than B601450 228-6655
455FE10 | B601455 | 228-8673 Sunplast Red |  | 0.1 | FCM
456FE01 | B601456 | 234-0077 SUNBRITE RED 2B 48:2 | PR 48:2 | 0.01 | FCM | 3C-6245, 399417 / C10 | 240 | Medium (6 months) | NON-FDA, [NAME] | BLUE | 8-10% | DO OT USE FOR PP IM APPLICATIONS. POSSIBLE FREE RADICAL REACTION
456FE10 | B601456 | 234-0077 SUNBRITE RED 2B 48:2 |  | 0.1 | FCM | 3C-6245, 3C-6295 / C9
456HE01 | B601456 | 234-0077 SUNBRITE RED 2B 48:2 |  | 0.01 | HIDM | 3C-6245 / C10
456HE10 | B601456 | 234-0077 SUNBRITE RED 2B 48:2 |  | 0.1 | HIDM
456HM01 | B601456 | 234-0077 SUNBRITE RED 2B 48:2 |  | 0.01 | HIDM
456HM10 | B601456 | 234-0077 SUNBRITE RED 2B 48:2 |  | 0.1 | HIDM | 3C-6245 / C10
140LC004 | 140LC004 | 5% Dryblend Intermediate 234-0077 |  | 0.05 | Powder Intermediate
457FE10 | D-B601457 | D-Bayplast Red GG | PR 48:1 | 0.1 | FCM | [PHONE] / C11 | 250 | Medium (6 months) | [NAME] | Yellow | 8 - 10% | **DO NOT USE - USE  - USE B601490**Same color as B601425 Red 2BY but cost less.
457HE10 | D-B601457 | D-Bayplast Red GG |  | 0.1 | HIDM | C11
458HE10 | D-B601458 | D-Bayplus Red BBC | PR 48:2 | 0.1 | HIDM | C11 | 240 | Medium (6 months) | Non FDA, [NAME] | blue | 10-12% | *USE B601490 INSTEAD*
N/A | D-B601459 | D-Spectrum Red 2Y | PR 48:3 | N/A | N/A |  | 240 | Medium | Non FDA, [NAME] | Blue | 10-12 | *DONOT USE*
461HE01 | D-B601461 | D-Colortherm 160M Red | PR 101 | 0.01 | HIDM | [PHONE] / C11 | 1000 | high | FDA, [NAME] | blue | 50% | Bluer than B601433 Red 120NM but yellower than B601462 Red 180M *DISCONTINEUD USE B601473 INSTEAD*
461HE10 | D-B601461 | D-Colortherm 160M Red |  | 0.1 | HIDM
462FE01 | D-B601462 | D-Bayferrox 180M Red | PR 101 | 0.01 | FCM |  | 1000 | high | FDA, [NAME] | blue | 50% | Slightly bluer than red B601401 *DISCONTINUED USE B601474 INSTEAD*
462HE01 | D-B601462 | D-Bayferrox 180M Red |  | 0.01 | HIDM
462HE10 | D-B601462 | D-Bayferrox 180M Red |  | 0.1 | HIDM | C11
462HE20 | D-B601462 | D-Bayferrox 180M Red |  | 0.2 | HIDM | CH7017392 / C12
463FS01 | D-B601463 | D-Red Iron Oxide 1550 | R101 | 0.01 | FCM |  | 1000 | High | [NAME] | Yellow | 50% | Same color as red 110M & 120NM but less than half cost. *USE B60173 INSTEAD*
463HE01 | D-B601463 | D-Red Iron Oxide 1550 |  | 0.01 | HIDM | 20041118-2 / C12
463HE20 | D-B601463 | D-Red Iron Oxide 1550 |  | 0.2 | HIDM
463HS01 | D-B601463 | D-Red Iron Oxide 1550 |  | 0.01 | HIDM | C12
466HE01 | D-B601466 | D-C14-6623 D&C Red #28 AL |  | 0.01 | HIDM | C12
467FE01 | B601467 | C19-7711 D&C Red#7 [NAME] | FD&C Red #7 | 0.01 | FCM | 5A3238 / C13 | 230 | poor | FDA, [NAME] | blue | 6-8% | HIGH MOISTURE CONTENT - DO NOT USE AT GREATER THAN 8% IN FORMULAS  **IF NOT AVAILABLE, USE B601446**
467FE10 | B601467 | C19-7711 D&C Red#7 [NAME] |  | 0.1 | FCM
467HE01 | B601467 | C19-7711 D&C Red#7 [NAME] |  | 0.01 | HIDM
471HE01 | B601471 | Nubiola R-5520 | PR 101 | 0.01 | HIDM |  |  |  |  |  |  | ** TO BE USED FOR FILM APPLICATION ONLY**
471HE10 | B601471 | Nubiola R-5520 | PR 101 | 0.1 | HIDM | C13 | 600 | High | FDA, [NAME] | yellow | 0.4
471HE20 | B601471 | Nubiola R-5520 |  | 0.2 | HIDM | C13
140LC013 | 140LC013 | Nubiola R-5520 Dryblend Intermediate |  | 0.05 | Powder Intermediate
472FE20 | B601472 | RED  IO. R 2521 | PR 101 | 0.2 | FCM | C14 | 600 | HIGH | FDA, [NAME] | Yellow | 40-50% | ** DO NOT USE FOR FILM APPLICATION** USE B601471 FOR FILM
472HE01 | B601472 | RED  IO. R 2521 |  | 0.01 | HIDM | 10/29/08 / C14
472HE20 | B601472 | RED  IO. R 2521 |  | 0.2 | HIDM
140LC006 | 140LC006 | RED IO  R- 2521 DRYBLEND |  | 0.05 | Powder Intermediate
473FE01 | B601473 | RED IO. R 2581 | PR 101 | 0.01 | FCM | STD / C14 | 600 | High | FDA, [NAME] | Blue | 40-50% | ** DO NOT USE FOR FILM APPLICATION** USE B601474 FOR FILM
473FE20 | B601473 | RED IO. R 2581 |  | 0.2 | FCM
473HE01 | B601473 | RED IO. R 2581 |  | 0.01 | HIDM
473HE20 | B601473 | RED IO. R 2581 |  | 0.2 | HIDM
140LC007 | 140LC007 | RED  IO  R-2581 [NAME] |  | 0.05 | Powder Intermediate
474FE01 | B601474 | RED IO. R 5580 | PR-101 | 0.01 | HIDM | STD / C14 | 600 | High | FDA, [NAME] | Yellow | 40-50% | ** TO BE USED FOR FILM APPLICATION ONLY**
474FE10 | B601474 | RED IO. R 5580 |  | 0.1 | HIDM
474FE20 | B601474 | RED IO. R 5580 |  | 0.2 | HIDM | STD / C15
474HE10 | B601474 | RED IO. R 5580 |  | 0.1 | HIDM
475FS05 | B601475 | MACROLEX RED EG |  | 0.05 | FCM | CHZTRD640/0709 | 280-300 depending on host resin | High | FDA for PET & PS only
477FE01 | B601477 | Keyplast Red Lake C | PR 101 | 0.01 | FCM | C15 | 260 | LOW | [NAME] | YELLow | 10-12% | ALWAYS USE 1.5% ZnSt FOR LOADINGS GREATER THAN 8%
477FE10 | B601477 | Keyplast Red Lake C |  | 0.1 | FCM
477HE01 | B601477 | Keyplast Red Lake C |  | 0.01 | HIDM | A208C331 / C15
477HE10 | B601477 | Keyplast Red Lake C |  | 0.1 | HIDM
140LC008 | 140LC008 | Keyplast Red Lake C Dryblend Intermediate |  | 0.05 | Powder Intermediate
478FE20 | B601478 | PREDISOL RED 3315-9 |  | 0.2 | FCM | Lot # DEDK 0010/0110 |  |  | [NAME]
478FE10 | B601478 | PREDISOL RED 3315-9 |  | 0.1 | FCM
478HE20 | B601478 | PREDISOL RED 3315-9 |  | 0.2 | HIDM
478HE10 | B601478 | PREDISOL RED 3315-9 |  | 0.1 | HIDM
487HE01 | [NAME] | Red IO  R- 2521 | PR 101 | 0.01 | HIDM | Std Lot | 600 | High | FDA, [NAME] | Yellow | 40-50% | **DO NOT USE FOR FILM** **USE TO REPLACE B601432 & B601433** YELLOWER THAN B601471/B601472
487HE20 | [NAME] | Red R-2512 | PR 101 | 0.2 | HIDM | Std Lot
488HE25 | B601488 | BNF-PK511 PINK FLUORESCENT |  | 0.25 | HIDM | 2-0811-0480-0609
488HE10 | B601488 | BNF-PK511 PINK FLUORESCENT |  | 0.1 | HIDM | 2-0811-0480-0609
140LC011 | 140LC011 | Red R-2512 Dryblend Intermediate |  | 0.05 | Powder Intermediate | Std Lot
490HE10 | B601490 | Red 234-3955 (48:1 2B) | 48:1 | 0.1 | HIDM | Master [NAME] | 240 | MEDIUM 6-8 MONTHS | [NAME] | YELLOW | 7-10%
490HE01 | B601490 | Red 234-3955 (48:1 2B) |  | 0.01 | HIDM | Master [NAME]
491HE10 | B601491 | Sun 228-5199 |  | 0.1 | HIDM | 4/12/06 / C17 | 260 | High | FDA, [NAME] | Blue |  | [NAME];  [NAME] than B601450
491HE01 | B601491 | Sun 228-5199 |  | 0.01 | HIDM
491FE10 | B601491 | Sun 228-5199 |  | 0.1 | FCM
491FE01 | B601491 | Sun 228-5199 |  | 0.01 | FCM
492HE10 | B601492 | Sun 234-7483 | 48:3 | 0.1 | HIDM |  | 250 | MEDIUM | [NAME] | BLUE | 8-12%
492HE01 | B601492 | Sun 234-7483 |  | 0.01 | HIDM
492FE10 | B601492 | Sun 234-7483 |  | 0.1 | FCM
492FE01 | B601492 | Sun 234-7483 |  | 0.01 | FCM
493FS10 | B601493 | [NAME] B |  | 0.1 | FCM
494HE25 | B601494 | [NAME] TZ40 |  | 0.25 | HIDM |  | 300 | High | FDA, [NAME] | Red | 0.25 | Maximum 25% loading
494HE10 | B601494 | [NAME] TZ40 |  | 0.1 | HIDM
494HE01 | B601494 | [NAME] TZ40 |  | 0.01 | HIDM
501FE01 | B601501 | Violet 8 Ultramarine | V15 | 0.01 | FCM
501FE10 | B601501 | Violet 8 Ultramarine |  | 0.1 | FCM |  | 280 | high | FDA | BLUE | 30-40% | THIS IS AN ULTRAMARINE VIOLET
501HE01 | B601501 | Violet 8 Ultramarine |  | 0.01 | HIDM
501HE10 | B601501 | Violet 8 Ultramarine |  | 0.1 | HIDM | 0721106 / C17
501HE25 | B601501 | Violet 8 Ultramarine |  | 0.25 | HIDM | 1090305 / C17
15900C18 | 15900C18 | VIOLET 8 DRY BLEND |  | 0.05 | Powder Intermediate
502FE01 | D-B601502 | D-Violet PL 3645(V23) | PV 23 | 0.01 | FCM | Jan./06 / C17 | 300 | high | Non FDA, [NAME] | blue | 8-10% | **DO NOT USE - USE B601508** 'Same color as B601503 but cost less than 1/2 the price
502FE10 | D-B601502 | D-Violet PL 3645(V23) |  | 0.1 | FCM | 18426-001 / C17
503FE10 | D-B601503 | D-246-4005 Indofast Violet | PV 23 | 0.1 | FCM | 74271-002 / C18 | 300 | High | Non-FDA, [NAME] | [NAME] | 8-10% | **DO NOT USE - USE B601508** High performance Pigment. Use only for critical injection molding or fiber application
504FE01 | D-B601504 | D-246-0505 Violet |  | 0.01 | FCM | C1CA01F0 / C18 |  |  |  |  |  | *DISCONTINUED DO NOT USE* USE B601508 INSTEAD.
504FE10 | D-B601504 | D-246-0505 Violet |  | 0.1 | FCM
504HE01 | D-B601504 | D-246-0505 Violet |  | 0.01 | HIDM
504HE10 | D-B601504 | D-246-0505 Violet |  | 0.1 | HIDM
N/A | D-B601505 | D-Tricolith Violet BLN | P.V. 23 | N/A | N/A |  | 300 | High | Non-FDA, [NAME] | Blue | 7-9% | DO NOT USE THIS PIGMENT.Similar to PV 19 from Bayer
N/A | D-B601510 | D-Magenta G | 122 | N/A | N/A |  | 280 | High | Non-FDA, [NAME] | Blue | 8-10% | DO NOT USE THIS PIGMENT. Use Bayer Magenta ERV-8655
N/A | D-B601512 | D-RV-6946-P Quindo Violet | P.V. 19 | N/A | N/A |  | 300 | High | FDA, [NAME] | Blue | 6-8% | DO NOT USE THIS PIGMENT. DISCONTINUED. USE BAYER ER-8672 B601452
508FE10 | B601508 | 246 ORKN Violet23 | PV 23 | 0.1 | FCM |  | 300 | HIGH | NON-FDA, [NAME] | BLUE/RED | 8-10%
508FE01 | B601508 | 246 ORKN Violet23 |  | 0.01 | FCM
513HE10 | B601513 | [NAME] Magenta |  | 0.1 | HIDM | T09JUL10-0809
513HE25 | B601513 | [NAME] Magenta | N/A | 0.25 | HIDM | T09JUL10-0809 | 280 | LOW | NON-FDA, [NAME] | BLUE | 15-25% | DO NOT USE
513HM10 | B601513 | [NAME] Magenta |  | 0.1 | HIDM | TONOV1 / C19
N/A | D-B601520 | D-NX-21 Magenta Fluorescent | NA | N/A | N/A |  | 200 | Poor | Non-FDA | Blue | 20% | DO NOT USE THIS PIGMENT. PIGMENT HAS BEEN DISCONTINUED
600FE01 | B601600 | K7090 Heliogen Blue | 15:3 | 0.01 | FCM | 60-7736, 080055P050/0708 / C21 | 280 | High | FDA, [NAME] | Green | 6-8% | Use B601610 when higher loading is needed. Similar to Bayer 2002-GP Blue. For IM application, add 10-20% B800501 Zeospheres W210 depend of the amount of this pigment in formula to prevent warping.                     **IF NOT AVAILABLE, USE B601654**
600FE10 | B601600 | K7090 Heliogen Blue |  | 0.1 | FCM | 080055P050/0708, 070092P050/0408 / C21
600HE01 | B601600 | K7090 Heliogen Blue |  | 0.01 | HIDM | 040025P050 / C21
600HE10 | B601600 | K7090 Heliogen Blue |  | 0.1 | HIDM
600FS05 | B601600 | K7090 Heliogen Blue |  | 0.05 | FCM | 80055P050/C21
160LC005 | 160LC005 | BLUE K7090 DRY BLEND |  | 0.05 | Powder Intermediate
N/A | D-B601601 | D-UMB DP 1160 Ultramarine Blue | B29 | N/A | N/A |  | 280 | High | FDA, [NAME] | Red | 40-50% | Red Shade Inorganic Blue. Similar to B601602 UMB 350. It does not promote warping.
602FE01 | D-B601602 | D-EP-37D / CM2047 UMB | B29 | 0.01 | FCM | Jan./06 / C21 | 280 | High | FDA, [NAME] | Red | 40-50% | Same colour as B601601. It does not promote warping. May cause moisture problems *USE B601647 INSTEAD*
602FE10 | D-B601602 | D-EP-37D / CM2047 UMB |  | 0.1 | FCM
602FE25 | D-B601602 | D-EP-37D / CM2047 UMB |  | 0.25 | FCM
602FE50 | D-B601602 | D-EP-37D / CM2047 UMB |  | 0.5 | FCM
602HE10 | D-B601602 | D-EP-37D / CM2047 UMB |  | 0.1 | HIDM | 072131 / C22
602HE25 | D-B601602 | D-EP-37D / CM2047 UMB |  | 0.25 | HIDM
602HE50 | D-B601602 | D-EP-37D / CM2047 UMB |  | 0.5 | HIDM
602HS10 | D-B601602 | D-EP-37D / CM2047 UMB |  | 0.1 | HIDM
16929C18 | D-16929C18 | D-UMB350 DRY BLEND | B29 | 0.05 | Powder Intermediate |  | 280 | High | FDA,[NAME] | Red | 40-50%
N/A | D-B601604 | D-C7084DD Heliogen Blue | 15:3 | N/A | N/A |  | 280 | High | FDA, [NAME] | Green | 6-8% | DO NOT USE THIS PIGMENT. USE B601600 or B601617
605FE01 | B601605 | L49-0714 PE Blue 15:3 (Flush) | 15:3 | 0.01 | FCM | D34703 / C22 | 260 | High | FDA, [NAME] | Green | 20-25% | Predispersed product with 50% pigment loading. Use in combination with Bayer B601617. Use when excellent pigment dispersion is required. For IM application add 10-20% of B800501 Zeoospheres W-210 depend the amount of this pigment in formula to prevent warping.
605FE10 | B601605 | L49-0714 PE Blue 15:3 (Flush) |  | 0.1 | FCM | D56411 / C22
605FE25 | B601605 | L49-0714 PE Blue 15:3 (Flush) |  | 0.25 | FCM
606FE10 | B601606 | 69-2001 Eupolen Blue | 15:1 | 0.1 | FCM | 060061P040 / C23 | 300 | High | FDA, [NAME] | Red | 20-25% | Predispersed product with 50% pigment loading. Use in combination with B601607 or B601612. Use when excellent pigment dispersion is required.For IM application add 10-20% of B800501 Zeoospheres W-210 depend the amount of this pigment in formula to prevent warping.
607FE01 | D-B601607 | D-K6911D Heliogen Blue | 15:1 | 0.01 | FCM | 51645000 / C23 | 300 | High | FDA, [NAME] | Red | 6-8% | Red shade Phthalo Blue. Similar to Bayplus Blue B. Use in combination with B601606 when maximum loading has been reached.For IM application add 10-20% of B800501 Zeoospheres W-210 depend the amount of this pigment in formula to prevent warping.
607FE08 | D-B601607 | D-K6911D Heliogen Blue |  | 0.08 | FCM | 84218 / C23
607FE10 | D-B601607 | D-K6911D Heliogen Blue |  | 0.1 | FCM | 51645000 / C23
N/A | D-B601608 | D-UMB 382-CP68 Ultramarine Blue | B29 | N/A | N/A |  | 280 | High | FDA, [NAME] | Green | 40-50% | DO NOT USE THIS PIGMENT. Use B601643 OR B601638
610FE10 | B601610 | 70-9001 Eupolen Blue (Flush) | 15:3 | 0.1 | FCM | 040007P040 / C24 | 280 | High | FDA, [NAME] | Green | 20-25% | Predispersed product with 50% pigment loading. Use in combination with B601600 or B601617. Use when excellent pigment dispersion is required.For IM application add 10-20% of B800501 Zeoospheres W-210 depend the amount of this pigment in formula to prevent warping.
N/A | D-B601611 | D-248-3745 Sunfast Blue 15:1 | PB 15:1 | N/A | N/A |  | 300 | high | FDA, [NAME] | red | 10-12% | For IM application add 10-20% of B800501 Zeoospheres W-210 depend the amount of this pigment in formula to prevent warping.
N/A | D-B601612 | D-Bayplus Blue B | 15:1 | N/A | N/A |  | 300 | High | FDA, [NAME] | Red | 6-8% | *USE B601635 INSTEAD*  Red shade Phthalo Blue. Similar to K6911 Heliogen Blue. Use in combination with B601606 when maximum loading has been reached.For IM application add 10-20% of B800501 Zeoospheres W-210 depend the amount of this pigment in formula to prevent warping.
N/A | D-B601614 | D-Microlen Blue 119 (Flush) | 15:1 | N/A | N/A |  | 260 | High | FDA, [NAME] | Red | 20-25% | DO NOT USE THIS PIGMENT. Use B601606 69-2001 Eupolen Blue
615HE50 | D-B601615 | D-Tricolith Blue BGS | 15:3 | N/A | N/A | 010711043 / C24 | 280 | High | FDA, [NAME] | Green | 6-8% | *DO NOT USE* DISCONTINUED. Use B601600 or B601617
N/A | D-B601616 | D-Tricolith Blue BR | 15:3 | N/A | N/A |  | 280 | High | FDA, Heavy Metal Pigment | Green | 6-8% | DO NOT USE THIS PIGMENT. PIGMENT HAS BEEN DISCONTINUED. Use B601600 or B601617
617FE01 | D-B601617 | D-Bayplus Blue 2002-GP | 15:3 | 0.01 | FCM | Jan./06 / C24 | 280 | High | FDA, [NAME] | Green | 6-8% | Similar to B601600 K7090. Use in combination with B601605 when excellent dispersion is required.For IM application add 10-20% of B800501 Zeoospheres W-210 depend the amount of this pigment in formula to prevent warping.
617FE08 | D-B601617 | D-Bayplus Blue 2002-GP |  | 0.08 | FCM | C24
617FV01 | D-B601617 | D-Bayplus Blue 2002-GP |  | 0.01 | FCM | 061116 / D1
617FV10 | D-B601617 | D-Bayplus Blue 2002-GP |  | 0.1 | FCM
617HE01 | D-B601617 | D-Bayplus Blue 2002-GP |  | 0.01 | HIDM | 061116 / D2
617HE10 | D-B601617 | D-Bayplus Blue 2002-GP |  | 0.1 | HIDM
617HS01 | D-B601617 | D-Bayplus Blue 2002-GP |  | 0.01 | HIDM | C24
618FE01 | D-B601618 | D-Blue 2764 | 15:1 | 0.01 | FCM | Jan./06 / D3 | 300 | High | FDA, [NAME] | Red | 6 -8% | *Use B601643 or B601638 instead* DONOT use this pigment is discontinued.
618FE10 | D-B601618 | D-Blue 2764 |  | 0.1 | FCM | 07-110 / D3
618FM10 | D-B601618 | D-Blue 2764 |  | 0.1 | FCM
618HE01 | D-B601618 | D-Blue 2764 |  | 0.01 | HIDM
618HE10 | D-B601618 | D-Blue 2764 |  | 0.1 | HIDM
618HS01 | D-B601618 | D-Blue 2764 |  | 0.01 | HIDM
618HS10 | D-B601618 | D-Blue 2764 |  | 0.1 | HIDM | D3
619FE01 | D-B601619 | D-Premiere DGS Ultramarine Blue | B29 | 0.01 | FCM | Jan./06 / D4 | 280 | High | FDA, [NAME] | Green | 0.4 | Greenest Ultramarine blue. Use when warping is a problem. *DISCONTINUED DO NOT USE* USE B601636 INSTEAD
619FE10 | D-B601619 | D-Premiere DGS Ultramarine Blue |  | 0.1 | FCM
619HE01 | D-B601619 | D-Premiere DGS Ultramarine Blue |  | 0.01 | HIDM
619HE10 | D-B601619 | D-Premiere DGS Ultramarine Blue |  | 0.1 | HIDM | D4
N/A | B601620 | Colbalt Blue 3 | N/A | N/A | N/A
N/A | D-B601621 | D-UMB Grade 02 | N/A | N/A | N/A
N/A | B601622 | 09901 FD&C Blue #1 Lake | FD &C Blue #1 | N/A | N/A |  | 218 | poor | FDA, [NAME] | green | 10-12% | Do not use unless specified
624HE10 | B601624 | [NAME] | N/A | 0.1 | HIDM | D4 | 300 | high | [NAME] | red | 50% | Only use for Kodak formulations
624HE20 | B601624 | [NAME] |  | 0.2 | HIDM | D5
624FE142 | B601624 | [NAME] |  | 0.142 | FCM | D4 |  |  |  |  |  | AKA: 16917-08 Blue Intermediate for 11622-08
625FE01 | B601625 | L48-3747 Blue 15:1(flush) | PB 15:1 | 0.01 | FCM | D83402 / D5 | 300 | high | FDA, [NAME] | red | 20-25% | Pre-dispersed product with 50% pigment loading of B601611.  For IM application add 10-20% of B800501 Zeoospheres W-210 depend the amount of this pigment in formula to prevent warping.
625FE10 | B601625 | L48-3747 Blue 15:1(flush) |  | 0.1 | FCM
625FE25 | B601625 | L48-3747 Blue 15:1(flush) |  | 0.25 | FCM | 10/29/07 / D6
N/A | B601626 | C39-4433 FD& C Blue#1 | FD& C Blue#1 | N/A | N/A |  | 218 | low | FDA, [NAME] | green | 10-12% | Do not use unless specified
628HE50 | D-B601628 | D-Premier FRX Ultramarine Blue | PB 29 | 0.5 | HIDM | 25426 / D6 | 280 | High | FDA | Red | 50 | this pigment is for Kodak formulations only(replaced B601624)
629FE01 | D-B601629 | D-HEUCO BLUE 515303 | 15:3 | 0.01 | FCM | 8L185 / D6 | 280 | high | [NAME] | Green | 6-8% | Donot use. Use B601600 instead.
629FE10 | D-B601629 | D-HEUCO BLUE 515303 |  | 0.1 | FCM | 8L185 / D7
630HE01 | B601630 | Nubiperf H56 Ultramarine Blue | N/A | 0.01 | HIDM | 1351104A / D7 | 280 | high | FDA, [NAME] | Medium | 70 | Use for high loading UMB application. 30% stronger than UMB 350 but not as  red as UMB 350
630HE10 | B601630 | Nubiperf H56 Ultramarine Blue |  | 0.1 | HIDM | D7
630HE50 | B601630 | Nubiperf H56 Ultramarine Blue |  | 0.5 | HIDM | 1351104A / D7
631HE01 | B601631 | Nubiperf FG75 Ultramarine Blue | N/A | 0.01 | HIDM | D8 | 280 | high | FDA, [NAME] | Green | 70 | Use for high loading Ultramarine blue application aprox. 30% stronger than B601619 UMB DGS .
631HE10 | B601631 | Nubiperf FG75 Ultramarine Blue |  | 0.1 | HIDM | 1780204A / D8
N/A | B601632 | Keyplast Blue A(206-036-51) | Solvent Blue 36 | N/A | N/A |  | 260 | Medium | [NAME] | Red | <10
635FE01 | D-B601635 | D-Bayplus Blue 716SD | 15:1 | 0.01 | FCM | Jan./06 / D8 | 300 | high | FDA, [NAME] | Red | 6-8 | Same color as B601618 Blue 2764(discontinued)but 30% stronger. For IM application add 10-20% of B800501 Zeoospheres W-210 depend the amount of this pigment
636FE01 | B601636 | Nubix C-84 UMB | B29 | 0.01 | FCM | STD / D8 | 260 | HIGH | FDA. HMF | GREEN | 0.4
[NAME] | B601636 | Nubix C-84 UMB |  | 0.1 | FCM | STD, 10/2/06 / D9
636FE25 | B601636 | Nubix C-84 UMB |  | 0.25 | FCM | STD / D9
636HE01 | B601636 | Nubix C-84 UMB |  | 0.01 | HIDM
636HE10 | B601636 | Nubix C-84 UMB |  | 0.1 | HIDM | D9
160LC013 | 160LC013 | Nubix C-84 UMB Dryblend Intermediate |  | 0.05 | Powder Intermediate
638HE01 | B601638 | 248-3700 BLUE | 15:1 | 0.01 | HIDM | Z76IN4256/0608 / D9 | 300 | HIGH | FDA, [NAME] | RED | 8-10%
638HE10 | B601638 | 248-3700 BLUE |  | 0.1 | HIDM | Z76IN4256/0608 / D11
638FE01 | B601638 | 248-3700 BLUE |  | 0.01 | FCM | Z33771, Z76IN4256/0608 / D10
638FE10 | B601638 | 248-3700 BLUE |  | 0.1 | FCM | Z251N4280, Z76IN4256/0608 / D10
639HE10 | B601639 | Macrolex Blue 3R | N/A | 0.1 | HIDM
643FE01 | B601643 | BLUE K6903 | 15:1 | 0.01 | FCM | 081604P050 / D11 | 300 | HIGH | FDA, [NAME] | RED | 8-10%
643FE10 | B601643 | BLUE K6903 |  | 0.1 | FCM
643HE01 | B601643 | BLUE K6903 |  | 0.01 | HIDM
643HE10 | B601643 | BLUE K6903 |  | 0.1 | HIDM | 081604P050 / D12
160LC010 | 160LC010 | 5%DB INTERM. BLUE K6903 |  | 1 | DB
644FS05 | B601644 | [NAME] |  | 0.05 | FCM |  | 280 - 300 depending  on the host resin | High | FDA for PET only
647FE01 | B601647 | Nubix E37 UMB | B29 | 0.01 | FCM |  | 260 | HIGH | FDA, [NAME] | RED | 0.4 | **USE THIS PIGMENT FOR TINT (i.e. SAME ARTIO WITH [NAME] OR LOWER) APPLICATIONS ONLY. THIS PIGMENT HAS NO COLOUR TOLERANCE IN MASSTONE, AND THEREFORE MUST ONLY BE USED IN COMBINATION WITH WHITE
647FE10 | B601647 | Nubix E37 UMB |  | 0.1 | FCM | STD / D12
647FE25 | B601647 | Nubix E37 UMB |  | 0.25 | FCM
647HE25 | B601647 | Nubix E37 UMB |  | 0.25 | HIDM
647FS01 | B601647 | Nubix E37 UMB |  | 0.01 | FCM
647FS10 | B601647 | Nubix E37 UMB |  | 0.1 | FCM
160LC014 | 160LC014 | Nubix E37 UMB Dryblend Intermediate |  | 0.05 | Powder Intermediate
648HE25 | D-B601648 | D-UMB LS285 | B29 | 0.25 | HIDM | 12/4/07 / D13
649HE10 | D-B601649 | D-Nubiola AR UMB | B29 | 0.1 | HIDM | 0711043,81604A / D13
649HE50 | D-B601649 | D-Nubiola AR UMB |  | 0.5 | HIDM | D13
652HE25 | B601652 | EP-37 Q2 UMB |  | 0.25 | HIDM |  | 260 | HIGH | FDA, [NAME] | RED | 0.4
652HE10 | B601652 | EP-37 Q2 UMB |  | 0.1
652HE01 | B601652 | EP-37 Q2 UMB |  | 0.01
160LC015 | 160LC015 | EP-37 Q2 ULTRAMARINE BLUE Dryblend Intermediate |  | 1 | Powder Intermediate
654FE10 | B601654 | 249-A80P Fastogen Blue |  | 0.1 | FCM |  |  |  |  |  |  | USE AS AN ALTERNATE TO B601600
654FE01 | B601654 | 249-A80P Fastogen Blue |  | 0.01 | FCM
654HE10 | B601654 | 249-A80P Fastogen Blue |  | 0.1 | HIDM
654HE01 | B601654 | 249-A80P Fastogen Blue |  | 0.15 | HIDM
700FE01 | D-'B601700 | D-'K8730 Heliogen Green | 7 | 0.01 | FCM | 16-4748, Jan./06 / D16 | >300 | High | NON-FDA, [NAME] | Blue | 8-10% | **DO NOT USE - USE B601707**Similar to B601712. Use in combination with B601708 when excellent diseprsion is required.  For IM application add 10-20% of B800501 Zeoospheres W-210 depend the amount of this pigment in formula to prevent warping.
700FE08 | D-'B601700 | D-'K8730 Heliogen Green |  | 0.08 | FCM
700FE10 | D-'B601700 | D-'K8730 Heliogen Green |  | 0.1 | FCM | D16
17901C18 | D-17901C18 | D-GREEN  K8730  DRY BLEND |  | 0.05 | Powder Intermediate
N/A | D-B601701 | D-D8605DD Heliogen Green | 7 | N/A | N/A |  | >300 | High | FDA, [NAME] | Blue | 7-10% | DO NOT USE THIS PIGMENT. Use B601700 or B601712
N/A | D-B601702 | D-PV Fast Green GNX | N/A | N/A | N/A
703HV01 | B601703 | [NAME] | N/A | 0.01 | HIDM | 8-3-04 / D16
703HV10 | B601703 | [NAME] |  | 0.1 | HIDM
703HV25 | B601703 | [NAME] |  | 0.25 | HIDM | D17
N/A | D-B601704 | D-6Y-FWC [NAME] | 36 | N/A | N/A |  | 260 | High | Non-FDA, [NAME] | Yellow | 7-10% | *DISCONTINUED* USE GREEN XGRE-6Y503 INSTEAD
N/A | D-B601705 | D-GLNP Irgalite Green | 7 | N/A | N/A |  | 300 | High | FDA, [NAME] | Blue | 7-10% | DO NOT USE THIS PIGMENT. Use B601700 or B601712
706FE01 | [NAME] | Lionol Green 6Y-503 | 36 | 0.01 | FCM | 30304, 7117 / D17 | 280 | HIGH | [NAME] | YELLOW | 7-10% | BROMINATED VERSION OF THE PG-7
706FE10 | [NAME] | Lionol Green 6Y-503 |  | 0.1 | FCM | 30304 / E1
707FE01 | D-B601707 | D-Heliogen Green K8730Z | 7 | 0.01 | FCM | 15677500, 081405P050, 81408P050 / E1 | 300 | HIGH | FDA,[NAME] | Blue | 8-10% | **DISCONTINUED** DO NOT USE; USE B601719 INSTEAD
707FE10 | D-B601707 | D-Heliogen Green K8730Z |  | 0.1 | FCM | 061415P05010507, 081405P050, 81408P050 / E1
707HE01 | D-B601707 | D-Heliogen Green K8730Z |  | 0.01 | HIDM | E1
707HE10 | D-B601707 | D-Heliogen Green K8730Z |  | 0.1 | HIDM | E2
170LC003 | D-170LC003 | D-GREEN K8730Z  DRY BLEND |  | 0.05 | Powder Intermediate
708FE01 | B601708 | 87-3001 Eupolen Green (Flush) | 7 | 0.01 | FCM | 69-3260 / E2 | 300 | High | FDA, [NAME] | Blue | 20-25% | Predispersed product with 50% pigment loading. Use in combination with B601700 or B601712. Use when excellent pigment dispersion is required.  For IM application add 10-20% of B800501 Zeoospheres W-210 depend the amount of this pigment in formula to prevent warping.
708FE10 | B601708 | 87-3001 Eupolen Green (Flush) |  | 0.1 | FCM
708FE25 | B601708 | 87-3001 Eupolen Green (Flush) |  | 0.25 | FCM | E3
708HE10 | B601708 | 87-3001 Eupolen Green (Flush) |  | 0.1 | HIDM | 050023P040 / E2
N/A | D-B601711 | D-Microlen GLNP Irgalite Green | 7 | N/A | N/A |  | 300 | High | FDA, [NAME] | Blue | 20-25% | DO NOT USE THIS PIGMENT. Use B601708
712FE01 | D-B601712 | D-Bayplus Green 2021 | 7 | 0.01 | FCM | 061211, Jan./06 / E4 | 300 | High | FDA, [NAME] | Blue | 7-10% | Similar to B601700. Use in combination with B601708 when excellent dispersion is required.  For IM application add 10-20% of B800501 Zeoospheres W-210 depend the amount of this pigment in formula to prevent warping. *DISCONTINUED USE B601707 INSTEAD*
712FE10 | D-B601712 | D-Bayplus Green 2021 |  | 0.1 | FCM | 061211, 18427-002 / E3
712HE01 | D-B601712 | D-Bayplus Green 2021 |  | 0.01 | HIDM | 061108, 061211 / E4
712HE10 | D-B601712 | D-Bayplus Green 2021 |  | 0.1 | HIDM | 061108 / E5
N/A | D-B601714 | D-GFNP Irgalite Green | 7 | N/A | N/A |  | 300 | High | FDA, [NAME] | Blue | 7-10% | DO NOT USE THIS PIGMENT.  Use B601700 or B601712
715FE01 | D-B601715 | D-GN-M Chrome Green | G17 | 0.01 | FCM | 137194, Jan./06 / E5 | 1000 | High | FDA, [NAME] | Blue | 40-45% | Extremelly wheatherable pigment. Weak and dirty typical to Inorganic pigments. FDA compliant to maximum of 5% pigment in the final product. *DISCONTINEUD DO NOT USE* USE B601716 INSTEAD
715FE15 | D-B601715 | D-GN-M Chrome Green |  | 0.15 | FCM
715HE01 | D-B601715 | D-GN-M Chrome Green |  | 0.01 | HIDM | E5
715HE15 | D-B601715 | D-GN-M Chrome Green |  | 0.15 | HIDM | E5
715HS10 | D-B601715 | D-GN-M Chrome Green |  | 0.1 | HIDM | E5
17902C18 | D-17902C18 | D-GREEN GNM DRY BLEND |  | 0.05 | Powder Intermediate
716HE20 | B601716 | Nubiocrom Green 2 | G17 | 0.2 | HIDM | 010751344 | 1000 | High | FDA, [NAME] | Blue | 40-45% | Extremelly wheatherable pigment. Weak and dirty typical to Inorganic pigments. FDA compliant to maximum of 5% pigment in the final product
716HE10 | B601716 | Nubiocrom Green 2 |  | 0.1 | HIDM | 010751344
716HE01 | B601716 | Nubiocrom Green 2 |  | 0.01 | HIDM | 010751344
170LC008 | 170LC008 | Nubiocrom Green 2 |  | 0.05 | Powder Intermediate
[NAME] | B601719 | 264-7700 Sunfast Green | 7 | 0.07 | FCM |  | 300 | HIGH | FDA, [NAME] | BLUE | 8-10%
719FE01 | B601719 | 264-7700 Sunfast Green |  | 0.01 | FCM
719HE07 | B601719 | 264-7700 Sunfast Green |  | 0.07 | HIDM
719HE01 | B601719 | 264-7700 Sunfast Green |  | 0.01 | HIDM
170LC010 | 170LC010 | 264-7700 Sunfast Green Dryblend Intermediate |  | 0.05 | Powder Intermediate
N/A | D-B601801 | D-Tan 20A Magnesium Ferrite | Y119 |  | N/A |  | 280 | High | Non-FDA, [NAME] | Red | 35-45% | *DISCONTINUED* Heat stable inorganic [NAME] pigment. Redder than B601803 and B601804. Try not to use unless absolutely necessary.
803HE10 | D-B601803 | D-Tan 10A Zinc Ferrite | Y119 | 0.1 | HIDM | E7 | 280 | High | Non-FDA, [NAME] | Midium Green | 35-45% | DO NOT USE THIS PIGMENT. Use B601804 Bayferrox 3950.
804FE01 | D-B601804 | D-Colortherm 3950 Zinc Ferrite | Y119 | 0.01 | FCM | Jan./06 / E7 | 270 | High | FDA, [NAME] | Medium Green | 35-45% | **USE ONLY FOR FDA APPLICATIONS - OTHERWISE USE B601805**'Heat stable yellow/tan pigment. If redder shade is needed, use in combination with Red 110 or 120 NM
804FE10 | D-B601804 | D-Colortherm 3950 Zinc Ferrite |  | 0.1 | FCM | CH710647510308 / E7
804HE10 | D-B601804 | D-Colortherm 3950 Zinc Ferrite |  | 0.1 | HIDM
804HE25 | D-B601804 | D-Colortherm 3950 Zinc Ferrite |  | 0.25 | HIDM | 10/29/08 / E7
804HS10 | D-B601804 | D-Colortherm 3950 Zinc Ferrite |  | 0.1 | HIDM | E7
805HE25 | B601805 | Yellow Y-905K |  | 0.25 | HIDM | 02094-2005-1209
805HE10 | B601805 | Yellow Y-905K |  | 0.1 | HIDM | 02094-2005-1209
805FE01 | B601805 | Yellow Y-905K |  | 0.01 | FCM | Standard / E8 | 260 | HIGH | FDA, [NAME] | MEDIUM - GREEN | 0.4
805FE25 | B601805 | Yellow Y-905K |  | 0.25 | FCM
180LC001 | 180LC001 | Yellow Y-905K Dryblend Intermediate |  | 0.05 | Powder Intermediate |  | 260
180LT031 | 180LT031 | Yellow Y-905K Pellet Intermediate |  | 0.05 | Pellet Intermediate |  | 260
N/A | B601900 | Cabot BP 160 (N660) | BL 7 | N/A | N/A |  | 600 | High | Non-FDA, [NAME] | Blue | 50%
901FE005 | D-B601901 | D-Cabot BP-120 (N762) | BL 7 | 0.005 | FCM |  | 600 | High | Non-FDA, [NAME] | Blue | 50% | **DISCONTINUED; DO NOT USE**  USE B601948                                                                           Use this pigment for matching colours. This is the  weakest of all the organic Blacks
901FE10 | D-B601901 | D-Cabot BP-120 (N762) |  | 0.1 | FCM
901HE005 | D-B601901 | D-Cabot BP-120 (N762) |  | 0.005 | HIDM | 2/13/06 / E11
901HE10 | D-B601901 | D-Cabot BP-120 (N762) |  | 0.1 | HIDM
901HE50 | D-B601901 | D-Cabot BP-120 (N762) |  | 0.5 | HIDM | E10
901HV01 | D-B601901 | D-Cabot BP-120 (N762) |  | 0.01 | HIDM | 709255, 790255 / E10
901HV10 | D-B601901 | D-Cabot BP-120 (N762) |  | 0.1 | HIDM
901HM10 | D-B601901 | D-Cabot BP-120 (N762) |  | 0.1 | HIDM
20951C18 | D-20951C18 | D-Black BP-120 Dryblend Intermediate |  | 0.05 | Powder Intermediate
902FE01 | B601902 | BK-4799 Black Iron Oxide | BL 11 | 0.01 | FCM |  | 220 | High | FDA, [NAME] | Blue | 30-40% | Weak pigment. Use for colormatching when heat stability is not a problem.
902HE01 | B601902 | BK-4799 Black Iron Oxide |  | 0.01 | HIDM | 2/13/06 / E11
902HE10 | B601902 | BK-4799 Black Iron Oxide |  | 0.1 | HIDM | E11
902HS01 | B601902 | BK-4799 Black Iron Oxide |  | 0.01 | HIDM | 12508105 / E11
20952C18 | 20952C18 | Black 4799 Dryblend Intermediate |  | 0.05 | Powder Intermediate
913HE10 | B601913 | BP-460(N330) [NAME] | N/A | 0.1 | HIDM | E11 |  |  | Non- FDA, [NAME]
917FE01 | B601917 | Arosperse 11 Carbon Black | N/A | 0.01 | FCM | [NAME] / E11 |  |  | Non-FDA, [NAME]
917FE10 | B601917 | Arosperse 11 Carbon Black |  | 0.1 | FCM | [NAME] / E12
923FE005 | D-B601923 | D-Cabot 4350 FDA Carbon Black | BL 7 | 0.005 | FCM |  | 600 | High | FDA, [NAME] | Blue | 40-50% | **DISCONTINUED; DO NOT USE - USE B601953**
923HE005 | D-B601923 | D-Cabot 4350 FDA Carbon Black |  | 0.005 | HIDM | 2/13/06 / E12
923HE01 | D-B601923 | D-Cabot 4350 FDA Carbon Black |  | 0.01 | HIDM | E12
923HE05 | D-B601923 | D-Cabot 4350 FDA Carbon Black |  | 0.05 | HIDM | E12
923HS005 | D-B601923 | D-Cabot 4350 FDA Carbon Black |  | 0.005 | HIDM | E12
923HS05 | D-B601923 | D-Cabot 4350 FDA Carbon Black |  | 0.05 | HIDM | E12
200LC022 | D-200LC022 | D-Black 4350 Dryblend Intermediate |  | 0.05 | Powder Intermediate
200LT022 | D-200LT022 | D-Black 4350 Dryblend Intermediated |  | 0.05 | Powder Intermediate
N/A | D-B601924 | D-Cabot 4750 FDA Carbon Black | BL 7 | N/A | N/A |  | 600 | High | FDA, [NAME] | Blue | 40-50% | FDA compliant up to 2.5% pigment in the final part. Stronger than B601923
934HE01 | D-B601934 | D-Silvet 220-20-E (Flush) | NA | 0.01 | HIDM | [NAME] | 280 | High | FDA, [NAME] | Metallic | 30% | **DISCONTINUED - DO NOT USE**  USE B601965 INSTEAD
934HE10 | D-B601934 | D-Silvet 220-20-E (Flush) |  | 0.1 | HIDM | 561584G / E13
934HE25 | D-B601934 | D-Silvet 220-20-E (Flush) |  | 0.25 | HIDM | 6CL63736 / E13
934HS01 | D-B601934 | D-Silvet 220-20-E (Flush) |  | 0.01 | HIDM
935HE10 | D-B601935 | D-Silvet 110-20-E | NA | 0.1 | HIDM | 5BL7834G / E13 | 280 | High | FDA, [NAME] | Metallic | 30% | Much cleaner than the 220-20-E. Does not flip as much as other large particle aluminum pigments.
N/A | D-B601936 | D-Silvet LT-1094 | NA | N/A | N/A | E14 | 280 | High | FDA, [NAME] | Metallic | 30% | Large particle aluminum flake.
937HE10 | D-B601937 | D-Sparkle Silvet 960-25-E | NA | 0.1 | HIDM | [NAME] |  |  |  |  |  | *DISCONTINUED DO NOT USE* USE B601959 INSTEAD
938HE25 | B601938 | Silvet 760-20-E | NA | 0.25 | HIDM | 0965403G0029 / E14 | 280 | High | Non-FDA, [NAME] | Metallic | 30% | DO NOT USE THIS PIGMENT. Use B601934 instead.
938HS10 | B601938 | Silvet 760-20-E |  | 0.1 | HIDM | 0GL4275 / E14
939HE10 | B601939 | Mastersafe 10203 | NA | 0.1 | HIDM | 10/29/08 / E14 | 280 | High | Non-FDA, [NAME] | Metallic | 0.3
940HE10 | D-B601940 | D-Silvet 880-20-E |  | 0.1 | HIDM |  |  |  |  |  |  | *DISCONTINUED DO NOT USE* USE B601960 INSTEAD
N/A | D-B601942 |  |  |  |  |  |  |  |  |  |  | *DISCONTINUED DO NOT USE* USE B601961 INSTEAD
948HE005 | [NAME] | N762 [NAME] | BL 7 | 0.005 | HIDM |  | 300 | HIGH | NON-FDA, [NAME] | YELLOW | 50%
948HE05 | [NAME] | N762 [NAME] |  | 0.05 | HIDM
948HE50 | [NAME] | Carbon Black N762 |  | 0.5 | HIDM | 06/19/09
200LC002 | 200LC002 | Black N762 Dryblend Intermediate |  | 0.05 | Powder Intermediate | 06/19/09
953HE005 | B601953 | Arosperse F138 (FDA) | BL 7 | 0.005 | HIDM |  | 300 | HIGH | FDA | BLUE | 0.35 | FDA compliant up to 2.5% pigment in the final part. Similar to the B601923
953HE05 | B601953 | Arosperse F138 (FDA) |  | 0.05 | HIDM
200LC023 | 200LC023 | Arosperse F138 (FDA) Dryblend Intermediate |  | 0.05 | Powder Intermediate | 7DL3128C / E14
N/A | B601954 | [NAME] 760-30-E1 | N/A | N/A | N/A | E15
955HE10 | D-B601955 | D-Silvex 440-15-C | N/A | 0.1 | HIDM |  |  |  |  |  |  | *DISCONTINUED DO NOT USE* USED B601962 INSTEAD
955HE25 | D-B601955 | D-Silvex 440-15-C |  | 0.25 | HIDM
959HE25 | B601959 | Eckart MP 15-20B | N/A | 0.25 | HIDM
959HE10 | B601959 | Eckart MP 15-20B |  | 0.1 | HIDM
959HE01 | B601959 | Eckart MP 15-20B |  | 0.01 | HIDM
960HE25 | B601960 | Eckart MP 29-20B | N/A | 0.25 | HIDM
960HE10 | B601960 | Eckart MP 29-20B |  | 0.1 | HIDM
960HE01 | B601960 | Eckart MP 29-20B |  | 0.01 | HIDM
961HE25 | B601961 | Eckart 20203 | N/A | 0.25 | HIDM
961HE10 | B601961 | Eckart 20203 |  | 0.1 | HIDM
961HE01 | B601961 | Eckart 20203 |  | 0.01 | HIDM
962HE25 | B601962 | Eckart MP85-20B | N/A | 0.25 | HIDM
962HE10 | B601962 | Eckart MP85-20B |  | 0.1 | HIDM
962HE01 | B601962 | Eckart MP85-20B |  | 0.01 | HIDM
963HE25 | D-B601963 | D-Eckart WM 1200 | N/A | 0.25 | HIDM |  |  |  |  |  |  | **DISCONTINUED - DO NOT USE**  USE B601965 INSTEAD
963HE10 | D-B601963 | D-Eckart WM 1200 |  | 0.1 | HIDM
963HE01 | D-B601963 | D-Eckart WM 1200 |  | 0.01 | HIDM
190LT031 | D-190LT031 | D-5% Eckart WM 1200 Pellet Intermediate |  | 0.05 | HIDM
965HE25 | B601965 | Stapa WM Chromal V/S/80 |  | 0.25 | HIDM
965HE10 | B601965 | Stapa WM Chromal V/S/80 |  | 0.1 | HIDM
965HE01 | B601965 | Stapa WM Chromal V/S/80 |  | 0.01 | HIDM
B800103 | B800103 | B900 Antioxidant | NA | 1 | A/O
B800111 | B800111 | Anox BB011 | NA | 1 | A/O
B800200 | B800200 | Sunovin 770/Tinuvin 770 (B800222) | NA | 1 | UV
B800203 | B800203 | Sunovin 944/Chimassorb 944FDL |  | 1 | UV
B800210 | B800210 | TINUVIN 783 HALS | NA | 1 | HALS
B800301 | B800301 | Armostat 300 (310) | NA | 1 | ANTISTAT
B800404 | B800404 | PE Wax | NA | 1 | WAX
B800428 | B800428 | [NAME] Wax | NA | 1 | Wax
501AE10 | B800501 | [NAME] | NA | 0.1 | Filler
B800501 | B800501 | [NAME] |  | 1 | ANTIWARP
507HE50 | B800507 | CaCO3 FT | N/A | 0.5 | HIDM
B800507 | B800507 | CaCO3 FT |  | 1 | Filler
507AE25 | B800507 | CaCO3 FT |  | 0.25 | Filler
507AE75 | B800507 | CaCO3 FT |  | 0.75 | Filler
534AE25 | B800534 | Calcium Sulfate | NA | 0.25 | Filler
535HE20 | B800535 | 9610 TALC | NA | 0.2 | HIDM
549AE25 | B800549 | Barium Sulfate | NA | 0.25 | Filler |  |  |  |  |  |  | Use B800559
642AE038 | B800642 | Hostalux KS-K | NA | 0.038 | Filler
B800702 | B800702 | [NAME] | NA | 1 | Zinc Stearate
B800703 | B800703 | CaSt | N/A | 1 | Calcium Stearate
B800540 | B800540 | OMYACARB 2SST | NA | 1 | FILLER
B800545 | B800545 | ZEOTHIX 265 | NA | 1 | FILLER
XBLA-PRINT60 | XBLA-PRINT60 | BLACK |  | 1